# Electronic Supplementary Material (ESI) for CrystEngComm.
# This journal is © The Royal Society of Chemistry 2018

####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_1
_database_code_depnum_ccdc_archive 'CCDC 1835435'
_audit_update_record             
;
2018-05-09 deposited with the CCDC.
2018-05-21 downloaded from the CCDC.
;

_audit_creation_method           SHELXL-97
_chemical_name_systematic        
; 
 ? 
;
_chemical_name_common            ?
_chemical_melting_point          ?
_chemical_formula_moiety         'C20 H32 As Co2 Mo8 N8 O40 V4'
_chemical_formula_sum            'C20 H32 As Co2 Mo8 N8 O40 V4'
_chemical_formula_weight         2187.61

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
V V 0.3005 0.5294 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Co Co 0.3494 0.9721 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
As As 0.0499 2.0058 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_H-M   'C 2/c'
_symmetry_space_group_name_Hall  '-C 2yc'
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, y, -z+1/2'
'x+1/2, y+1/2, z'
'-x+1/2, y+1/2, -z+1/2'
'-x, -y, -z'
'x, -y, z-1/2'
'-x+1/2, -y+1/2, -z'
'x+1/2, -y+1/2, z-1/2'

_cell_length_a                   12.3495(11)
_cell_length_b                   21.893(2)
_cell_length_c                   19.7759(18)
_cell_angle_alpha                90.00
_cell_angle_beta                 103.632(2)
_cell_angle_gamma                90.00
_cell_volume                     5196.1(8)
_cell_formula_units_Z            4
_cell_measurement_temperature    293(2)
_cell_measurement_reflns_used    4577
_cell_measurement_theta_min      1.86
_cell_measurement_theta_max      25.59

_exptl_crystal_description       block
_exptl_crystal_colour            blue
_exptl_crystal_size_max          0.19
_exptl_crystal_size_mid          0.18
_exptl_crystal_size_min          0.16
_exptl_crystal_density_meas      ?
_exptl_crystal_density_diffrn    2.782
_exptl_crystal_density_method    'not measured'
_exptl_crystal_F_000             4108
_exptl_absorpt_coefficient_mu    3.906
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_correction_T_min  0.481
_exptl_absorpt_correction_T_max  0.535
_exptl_absorpt_process_details   SADABS

_exptl_special_details           
; 
 ? 
;

_diffrn_ambient_temperature      293(2)
_diffrn_radiation_wavelength     0.71073
_diffrn_radiation_type           MoK\a
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_monochromator  graphite
_diffrn_measurement_device_type  'Bruker Smart APEX CCD area detector'
_diffrn_measurement_method       'phi and omega scans'
_diffrn_detector_area_resol_mean ?
_diffrn_standards_number         ?
_diffrn_standards_interval_count ?
_diffrn_standards_interval_time  ?
_diffrn_standards_decay_%        ?
_diffrn_reflns_number            15907
_diffrn_reflns_av_R_equivalents  0.0422
_diffrn_reflns_av_sigmaI/netI    0.0400
_diffrn_reflns_limit_h_min       -14
_diffrn_reflns_limit_h_max       14
_diffrn_reflns_limit_k_min       -26
_diffrn_reflns_limit_k_max       23
_diffrn_reflns_limit_l_min       -23
_diffrn_reflns_limit_l_max       20
_diffrn_reflns_theta_min         1.86
_diffrn_reflns_theta_max         25.09
_reflns_number_total             4577
_reflns_number_gt                3897
_reflns_threshold_expression     >2sigma(I)

_computing_data_collection       'Bruker SMART'
_computing_cell_refinement       'Bruker SMART'
_computing_data_reduction        'Bruker SAINT'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_molecular_graphics    SHELXP-97
_computing_publication_material  SHELXTL

_refine_special_details          
; 
 Refinement of F² against ALL reflections.  The weighted R-factor wR and 
 goodness of fit S are based on F², conventional R-factors R are based 
 on F, with F set to zero for negative F². The threshold expression of 
 F² > 2sigma(F²) is used only for calculating R-factors(gt) etc. and is 
 not relevant to the choice of reflections for refinement.  R-factors based 
 on F² are statistically about twice as large as those based on F, and R- 
 factors based on ALL data will be even larger. 
;

_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'calc w=1/[σ²(Fo²)+(0.0524P)²+81.2788P] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_atom_sites_solution_hydrogens   geom
_refine_ls_hydrogen_treatment    mixed
_refine_ls_extinction_method     none
_refine_ls_extinction_coef       ?
_refine_ls_number_reflns         4577
_refine_ls_number_parameters     393
_refine_ls_number_restraints     4
_refine_ls_R_factor_all          0.0496
_refine_ls_R_factor_gt           0.0408
_refine_ls_wR_factor_ref         0.1156
_refine_ls_wR_factor_gt          0.1097
_refine_ls_goodness_of_fit_ref   1.042
_refine_ls_restrained_S_all      1.048
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
As1 As 0.0000 0.42613(4) 0.2500 0.0147(2) Uani 1 2 d S . .
Mo4 Mo 0.29815(5) 0.43312(3) 0.30403(3) 0.02116(17) Uani 1 1 d . . .
Mo2 Mo -0.01752(5) 0.41972(3) 0.06818(3) 0.02091(17) Uani 1 1 d . . .
Mo3 Mo 0.14784(5) 0.54825(3) 0.19184(3) 0.02168(17) Uani 1 1 d . . .
Mo1 Mo 0.12994(5) 0.30421(3) 0.17823(3) 0.02084(17) Uani 1 1 d . . .
V2 V -0.15621(8) 0.54386(5) 0.13857(5) 0.0108(2) Uani 1 1 d . . .
V1 V -0.14547(9) 0.30932(5) 0.13463(5) 0.0142(2) Uani 1 1 d . . .
Co1 Co 0.24098(8) 0.42796(4) 0.14233(5) 0.0191(2) Uani 1 1 d . . .
O1 O 0.2832(4) 0.4880(2) 0.2168(3) 0.0235(11) Uani 1 1 d . . .
O2 O -0.0023(4) 0.3813(2) 0.1811(2) 0.0180(10) Uani 1 1 d . . .
O3 O 0.0007(4) 0.5634(2) 0.1682(3) 0.0247(11) Uani 1 1 d . . .
O4 O 0.1351(4) 0.2895(2) 0.2684(3) 0.0253(11) Uani 1 1 d . . .
O5 O -0.1087(4) 0.4779(2) 0.0865(2) 0.0245(11) Uani 1 1 d . . .
O6 O 0.2014(4) 0.5979(2) 0.1439(3) 0.0310(12) Uani 1 1 d . . .
O7 O -0.2316(4) 0.2599(2) 0.0935(3) 0.0280(12) Uani 1 1 d . . .
O8 O 0.2387(4) 0.3782(2) 0.2152(2) 0.0245(11) Uani 1 1 d . . .
O9 O 0.1199(4) 0.3622(2) 0.0949(2) 0.0236(11) Uani 1 1 d . . .
O10 O -0.0075(5) 0.4326(2) -0.0135(3) 0.0301(12) Uani 1 1 d . . .
O11 O -0.0034(4) 0.2692(2) 0.1390(2) 0.0236(11) Uani 1 1 d . . .
O12 O 0.4352(4) 0.4175(2) 0.3187(3) 0.0314(12) Uani 1 1 d . . .
O13 O -0.1132(4) 0.4708(2) 0.2321(2) 0.0196(10) Uani 1 1 d . . .
O14 O 0.1822(4) 0.5826(2) 0.2770(3) 0.0234(11) Uani 1 1 d . . .
O15 O -0.2049(4) 0.5938(2) 0.0797(3) 0.0312(12) Uani 1 1 d . . .
O16 O 0.2454(4) 0.3738(2) 0.3508(2) 0.0255(11) Uani 1 1 d . . .
O17 O 0.2209(4) 0.2548(3) 0.1574(3) 0.0325(13) Uani 1 1 d . . .
O18 O 0.1144(4) 0.4730(2) 0.1237(3) 0.0250(11) Uani 1 1 d . . .
O19 O -0.1143(4) 0.3550(2) 0.0568(2) 0.0245(11) Uani 1 1 d . . .
O20 O 0.2932(4) 0.4975(2) 0.3598(3) 0.0245(11) Uani 1 1 d . . .
N2 N 0.0828(7) 0.2837(4) 0.9807(4) 0.048(2) Uani 1 1 d . . .
H2A H 0.1152 0.3073 1.0141 0.058 Uiso 1 1 calc R . .
C1 C 0.0141(8) 0.3008(4) 0.9240(4) 0.039(2) Uani 1 1 d . . .
H1 H -0.0094 0.3408 0.9135 0.047 Uiso 1 1 calc R . .
C2 C 0.0953(10) 0.2222(5) 0.9785(6) 0.060(3) Uani 1 1 d . . .
H2 H 0.1388 0.1980 1.0131 0.073 Uiso 1 1 calc R . .
N1 N -0.0176(6) 0.2537(3) 0.8834(4) 0.0390(17) Uani 1 1 d . . .
C3 C 0.0344(10) 0.2034(4) 0.9183(5) 0.056(3) Uani 1 1 d . . .
H3 H 0.0276 0.1633 0.9023 0.068 Uiso 1 1 calc R . .
C4 C -0.0947(8) 0.2559(7) 0.8121(5) 0.070(4) Uani 1 1 d D . .
N4 N 0.9680(6) 0.1021(3) 0.1093(4) 0.0385(17) Uani 1 1 d . . .
N3 N 0.8250(6) 0.1092(4) 0.0260(4) 0.053(2) Uani 1 1 d . . .
H3A H 0.7705 0.1247 -0.0044 0.064 Uiso 1 1 calc R . .
C6 C 1.0607(8) 0.1181(5) 0.1696(5) 0.051(3) Uani 1 1 d D . .
C7 C 0.9423(9) 0.0440(5) 0.0832(6) 0.064(3) Uani 1 1 d . . .
H7 H 0.9811 0.0083 0.0989 0.077 Uiso 1 1 calc R . .
C8 C 0.8524(10) 0.0485(5) 0.0319(6) 0.068(3) Uani 1 1 d . . .
H8 H 0.8149 0.0167 0.0051 0.082 Uiso 1 1 calc R . .
C9 C 0.8937(7) 0.1394(5) 0.0732(5) 0.047(2) Uani 1 1 d . . .
H9 H 0.8909 0.1813 0.0805 0.056 Uiso 1 1 calc R . .
C5A C -0.0360(14) 0.2335(9) 0.7650(9) 0.061(7) Uani 0.50 1 d PD . .
C5B C -0.0456(13) 0.2815(8) 0.7618(8) 0.043(4) Uani 0.50 1 d PD . .
C10A C 1.0393(15) 0.1420(8) 0.2294(8) 0.042(4) Uani 0.50 1 d PD . .
C10B C 1.038(2) 0.1004(10) 0.2319(8) 0.083(11) Uani 0.50 1 d PD . .


_geom_special_details            
; 
 All esds (except the esd in the dihedral angle between two l.s. planes) 
 are estimated using the full covariance matrix.  The cell esds are taken 
 into account individually in the estimation of esds in distances, angles 
 and torsion angles; correlations between esds in cell parameters are only 
 used when they are defined by crystal symmetry.  An approximate (isotropic) 
 treatment of cell esds is used for estimating esds involving l.s. planes. 
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
As1 O13 1.674(4) . ?
As1 O13 1.674(4) 2 ?
As1 O2 1.674(4) . ?
As1 O2 1.674(4) 2 ?
Mo4 O12 1.684(5) . ?
Mo4 O20 1.800(5) . ?
Mo4 O16 1.803(5) . ?
Mo4 O1 2.074(5) . ?
Mo4 O8 2.114(5) . ?
Mo4 O13 2.374(4) 2 ?
Mo2 O10 1.673(5) . ?
Mo2 O5 1.793(5) . ?
Mo2 O19 1.833(5) . ?
Mo2 O9 2.079(5) . ?
Mo2 O18 2.093(5) . ?
Mo2 O2 2.351(5) . ?
Mo3 O6 1.677(5) . ?
Mo3 O3 1.797(5) . ?
Mo3 O14 1.801(5) . ?
Mo3 O1 2.095(5) . ?
Mo3 O18 2.106(5) . ?
Mo3 O13 2.371(5) 2 ?
Mo1 O17 1.680(5) . ?
Mo1 O4 1.799(5) . ?
Mo1 O11 1.816(5) . ?
Mo1 O9 2.060(5) . ?
Mo1 O8 2.120(5) . ?
Mo1 O2 2.359(5) . ?
V2 O15 1.607(5) . ?
V2 O3 1.935(5) . ?
V2 O5 1.942(5) . ?
V2 O14 1.965(5) 2 ?
V2 O20 1.979(5) 2 ?
V2 O13 2.409(5) . ?
V1 O7 1.598(5) . ?
V1 O4 1.940(5) 2 ?
V1 O16 1.941(5) 2 ?
V1 O11 1.945(5) . ?
V1 O19 1.948(5) . ?
V1 O2 2.386(4) . ?
Co1 O8 1.812(5) . ?
Co1 O18 1.812(5) . ?
Co1 O1 1.951(5) . ?
Co1 O9 2.129(5) . ?
O4 V1 1.940(5) 2 ?
O13 Mo3 2.371(5) 2 ?
O13 Mo4 2.374(4) 2 ?
O14 V2 1.965(5) 2 ?
O16 V1 1.941(5) 2 ?
O20 V2 1.980(5) 2 ?
N2 C1 1.291(11) . ?
N2 C2 1.357(13) . ?
N2 H2A 0.8600 . ?
C1 N1 1.309(11) . ?
C1 H1 0.9300 . ?
C2 C3 1.316(14) . ?
C2 H2 0.9300 . ?
N1 C3 1.376(13) . ?
N1 C4 1.506(12) . ?
C3 H3 0.9300 . ?
C4 C5A 1.397(10) . ?
C4 C5B 1.398(10) . ?
N4 C9 1.307(11) . ?
N4 C7 1.383(12) . ?
N4 C6 1.487(11) . ?
N3 C9 1.286(12) . ?
N3 C8 1.369(14) . ?
N3 H3A 0.8600 . ?
C6 C10A 1.374(9) . ?
C6 C10B 1.382(10) . ?
C7 C8 1.319(14) . ?
C7 H7 0.9300 . ?
C8 H8 0.9300 . ?
C9 H9 0.9300 . ?
C5A C5B 1.06(2) . ?
C5A C5A 1.18(3) 2_556 ?
C5A C5B 1.63(2) 2_556 ?
C5B C5B 1.32(3) 2_556 ?
C5B C5A 1.63(2) 2_556 ?
C10A C10B 0.91(2) . ?
C10A C10A 1.41(3) 2_755 ?
C10A C10B 1.63(2) 2_755 ?
C10B C10B 1.31(4) 2_755 ?
C10B C10A 1.63(2) 2_755 ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O13 As1 O13 108.6(3) . 2 ?
O13 As1 O2 108.5(2) . . ?
O13 As1 O2 111.5(2) 2 . ?
O13 As1 O2 111.5(2) . 2 ?
O13 As1 O2 108.5(2) 2 2 ?
O2 As1 O2 108.3(3) . 2 ?
O12 Mo4 O20 103.4(2) . . ?
O12 Mo4 O16 103.6(2) . . ?
O20 Mo4 O16 100.4(2) . . ?
O12 Mo4 O1 98.6(2) . . ?
O20 Mo4 O1 92.7(2) . . ?
O16 Mo4 O1 150.7(2) . . ?
O12 Mo4 O8 99.6(2) . . ?
O20 Mo4 O8 154.2(2) . . ?
O16 Mo4 O8 85.4(2) . . ?
O1 Mo4 O8 72.10(19) . . ?
O12 Mo4 O13 168.3(2) . 2 ?
O20 Mo4 O13 75.15(19) . 2 ?
O16 Mo4 O13 88.07(19) . 2 ?
O1 Mo4 O13 69.98(17) . 2 ?
O8 Mo4 O13 79.97(18) . 2 ?
O10 Mo2 O5 105.6(2) . . ?
O10 Mo2 O19 101.9(2) . . ?
O5 Mo2 O19 98.7(2) . . ?
O10 Mo2 O9 96.1(2) . . ?
O5 Mo2 O9 153.3(2) . . ?
O19 Mo2 O9 91.8(2) . . ?
O10 Mo2 O18 100.8(2) . . ?
O5 Mo2 O18 86.9(2) . . ?
O19 Mo2 O18 154.2(2) . . ?
O9 Mo2 O18 73.57(19) . . ?
O10 Mo2 O2 165.8(2) . . ?
O5 Mo2 O2 88.59(19) . . ?
O19 Mo2 O2 75.17(18) . . ?
O9 Mo2 O2 70.38(17) . . ?
O18 Mo2 O2 79.80(18) . . ?
O6 Mo3 O3 104.1(2) . . ?
O6 Mo3 O14 102.8(2) . . ?
O3 Mo3 O14 99.6(2) . . ?
O6 Mo3 O1 98.2(2) . . ?
O3 Mo3 O1 151.5(2) . . ?
O14 Mo3 O1 92.5(2) . . ?
O6 Mo3 O18 100.9(2) . . ?
O3 Mo3 O18 86.8(2) . . ?
O14 Mo3 O18 153.1(2) . . ?
O1 Mo3 O18 71.56(19) . . ?
O6 Mo3 O13 167.4(2) . 2 ?
O3 Mo3 O13 88.5(2) . 2 ?
O14 Mo3 O13 75.15(19) . 2 ?
O1 Mo3 O13 69.69(17) . 2 ?
O18 Mo3 O13 78.98(18) . 2 ?
O17 Mo1 O4 104.9(2) . . ?
O17 Mo1 O11 102.4(2) . . ?
O4 Mo1 O11 99.4(2) . . ?
O17 Mo1 O9 96.8(2) . . ?
O4 Mo1 O9 152.2(2) . . ?
O11 Mo1 O9 92.3(2) . . ?
O17 Mo1 O8 99.8(2) . . ?
O4 Mo1 O8 85.6(2) . . ?
O11 Mo1 O8 155.0(2) . . ?
O9 Mo1 O8 73.69(19) . . ?
O17 Mo1 O2 166.9(2) . . ?
O4 Mo1 O2 88.1(2) . . ?
O11 Mo1 O2 75.47(18) . . ?
O9 Mo1 O2 70.53(17) . . ?
O8 Mo1 O2 80.25(17) . . ?
O15 V2 O3 104.3(2) . . ?
O15 V2 O5 103.3(3) . . ?
O3 V2 O5 85.3(2) . . ?
O15 V2 O14 102.3(3) . 2 ?
O3 V2 O14 90.0(2) . 2 ?
O5 V2 O14 154.3(2) . 2 ?
O15 V2 O20 100.6(2) . 2 ?
O3 V2 O20 155.1(2) . 2 ?
O5 V2 O20 89.6(2) . 2 ?
O14 V2 O20 84.0(2) 2 2 ?
O15 V2 O13 170.2(2) . . ?
O3 V2 O13 83.71(19) . . ?
O5 V2 O13 82.75(19) . . ?
O14 V2 O13 71.61(18) 2 . ?
O20 V2 O13 71.42(17) 2 . ?
O7 V1 O4 103.4(2) . 2 ?
O7 V1 O16 101.4(2) . 2 ?
O4 V1 O16 85.0(2) 2 2 ?
O7 V1 O11 101.7(2) . . ?
O4 V1 O11 90.3(2) 2 . ?
O16 V1 O11 156.9(2) 2 . ?
O7 V1 O19 100.2(2) . . ?
O4 V1 O19 156.4(2) 2 . ?
O16 V1 O19 89.7(2) 2 . ?
O11 V1 O19 85.6(2) . . ?
O7 V1 O2 170.8(2) . . ?
O4 V1 O2 84.11(19) 2 . ?
O16 V1 O2 84.35(18) 2 . ?
O11 V1 O2 72.68(18) . . ?
O19 V1 O2 72.44(18) . . ?
O8 Co1 O18 108.4(2) . . ?
O8 Co1 O1 81.8(2) . . ?
O18 Co1 O1 81.4(2) . . ?
O8 Co1 O9 78.6(2) . . ?
O18 Co1 O9 78.2(2) . . ?
O1 Co1 O9 145.4(2) . . ?
Co1 O1 Mo4 101.2(2) . . ?
Co1 O1 Mo3 100.9(2) . . ?
Mo4 O1 Mo3 118.1(2) . . ?
As1 O2 Mo2 123.1(2) . . ?
As1 O2 Mo1 124.1(2) . . ?
Mo2 O2 Mo1 97.71(16) . . ?
As1 O2 V1 124.7(2) . . ?
Mo2 O2 V1 89.10(15) . . ?
Mo1 O2 V1 88.41(15) . . ?
Mo3 O3 V2 156.5(3) . . ?
Mo1 O4 V1 156.6(3) . 2 ?
Mo2 O5 V2 156.6(3) . . ?
Co1 O8 Mo4 104.5(2) . . ?
Co1 O8 Mo1 108.2(2) . . ?
Mo4 O8 Mo1 142.1(3) . . ?
Mo1 O9 Mo2 117.9(2) . . ?
Mo1 O9 Co1 99.23(19) . . ?
Mo2 O9 Co1 98.5(2) . . ?
Mo1 O11 V1 123.1(3) . . ?
As1 O13 Mo3 123.4(2) . 2 ?
As1 O13 Mo4 123.9(2) . 2 ?
Mo3 O13 Mo4 97.77(16) 2 2 ?
As1 O13 V2 124.9(2) . . ?
Mo3 O13 V2 88.37(16) 2 . ?
Mo4 O13 V2 88.68(15) 2 . ?
Mo3 O14 V2 124.4(3) . 2 ?
Mo4 O16 V1 156.8(3) . 2 ?
Co1 O18 Mo2 109.3(2) . . ?
Co1 O18 Mo3 105.4(2) . . ?
Mo2 O18 Mo3 141.5(2) . . ?
Mo2 O19 V1 123.0(2) . . ?
Mo4 O20 V2 124.3(3) . 2 ?
C1 N2 C2 108.4(8) . . ?
C1 N2 H2A 125.8 . . ?
C2 N2 H2A 125.8 . . ?
N2 C1 N1 110.2(8) . . ?
N2 C1 H1 124.9 . . ?
N1 C1 H1 124.9 . . ?
C3 C2 N2 107.1(10) . . ?
C3 C2 H2 126.4 . . ?
N2 C2 H2 126.4 . . ?
C1 N1 C3 106.7(8) . . ?
C1 N1 C4 125.5(9) . . ?
C3 N1 C4 127.8(8) . . ?
C2 C3 N1 107.6(9) . . ?
C2 C3 H3 126.2 . . ?
N1 C3 H3 126.2 . . ?
C5A C4 C5B 44.5(10) . . ?
C5A C4 N1 107.5(11) . . ?
C5B C4 N1 113.3(10) . . ?
C9 N4 C7 107.5(8) . . ?
C9 N4 C6 126.9(8) . . ?
C7 N4 C6 125.6(8) . . ?
C9 N3 C8 109.2(8) . . ?
C9 N3 H3A 125.4 . . ?
C8 N3 H3A 125.4 . . ?
C10A C6 C10B 38.7(10) . . ?
C10A C6 N4 120.8(11) . . ?
C10B C6 N4 111.6(13) . . ?
C8 C7 N4 107.2(9) . . ?
C8 C7 H7 126.4 . . ?
N4 C7 H7 126.4 . . ?
C7 C8 N3 106.5(9) . . ?
C7 C8 H8 126.7 . . ?
N3 C8 H8 126.7 . . ?
N3 C9 N4 109.5(9) . . ?
N3 C9 H9 125.2 . . ?
N4 C9 H9 125.2 . . ?
C5B C5A C5A 93.3(11) . 2_556 ?
C5B C5A C4 67.8(9) . . ?
C5A C5A C4 155.0(16) 2_556 . ?
C5B C5A C5B 53.8(13) . 2_556 ?
C5A C5A C5B 40.4(8) 2_556 2_556 ?
C4 C5A C5B 116.7(14) . 2_556 ?
C5A C5B C5B 85.8(11) . 2_556 ?
C5A C5B C4 67.7(8) . . ?
C5B C5B C4 143.3(16) 2_556 . ?
C5A C5B C5A 46.2(13) . 2_556 ?
C5B C5B C5A 40.4(7) 2_556 2_556 ?
C4 C5B C5A 112.1(14) . 2_556 ?
C10B C10A C6 71.2(9) . . ?
C10B C10A C10A 86.8(14) . 2_755 ?
C6 C10A C10A 142.9(18) . 2_755 ?
C10B C10A C10B 52.9(18) . 2_755 ?
C6 C10A C10B 116.3(14) . 2_755 ?
C10A C10A C10B 33.9(8) 2_755 2_755 ?
C10A C10B C10B 93.1(14) . 2_755 ?
C10A C10B C6 70.2(10) . . ?
C10B C10B C6 144(2) 2_755 . ?
C10A C10B C10A 59.3(14) . 2_755 ?
C10B C10B C10A 33.9(8) 2_755 2_755 ?
C6 C10B C10A 121.7(14) . 2_755 ?

loop_
_geom_hbond_atom_site_label_D
_geom_hbond_atom_site_label_H
_geom_hbond_atom_site_label_A
_geom_hbond_distance_DH
_geom_hbond_distance_HA
_geom_hbond_distance_DA
_geom_hbond_angle_DHA
_geom_hbond_site_symmetry_A
N2 H2A O9 0.86 1.99 2.788(9) 154.3 1_556
N3 H3A O19 0.86 2.01 2.839(9) 160.9 7

_diffrn_measured_fraction_theta_max 0.992
_diffrn_reflns_theta_full        25.09
_diffrn_measured_fraction_theta_full 0.992
_refine_diff_density_max         2.528
_refine_diff_density_min         -1.187
_refine_diff_density_rms         0.169

####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_2
_database_code_depnum_ccdc_archive 'CCDC 1835436'
_audit_update_record             
;
2018-05-09 deposited with the CCDC.
2018-05-21 downloaded from the CCDC.
;

_audit_creation_method           SHELXL-97
_chemical_name_systematic        
; 
 ? 
;
_chemical_name_common            ?
_chemical_melting_point          ?
_chemical_formula_moiety         'C50 H84 As2 Cu4 Mo16 N20 O83 V8'
_chemical_formula_sum            'C50 H84 As2 Cu4 Mo16 N20 O83 V8'
_chemical_formula_weight         4639.93

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cu Cu 0.3201 1.2651 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
As As 0.0499 2.0058 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Na Na 0.0362 0.0249 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
V V 0.3005 0.5294 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_symmetry_cell_setting           triclinic
_symmetry_space_group_name_H-M   'P -1'
_symmetry_space_group_name_Hall  '-P 1'
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, -z'

_cell_length_a                   10.733(4)
_cell_length_b                   13.361(4)
_cell_length_c                   21.952(7)
_cell_angle_alpha                89.302(6)
_cell_angle_beta                 79.585(6)
_cell_angle_gamma                75.901(5)
_cell_volume                     3001.1(17)
_cell_formula_units_Z            1
_cell_measurement_temperature    293(2)
_cell_measurement_reflns_used    10394
_cell_measurement_theta_min      0.94
_cell_measurement_theta_max      25.15

_exptl_crystal_description       block
_exptl_crystal_colour            blue
_exptl_crystal_size_max          0.22
_exptl_crystal_size_mid          0.19
_exptl_crystal_size_min          0.17
_exptl_crystal_density_meas      ?
_exptl_crystal_density_diffrn    2.567
_exptl_crystal_density_method    'not measured'
_exptl_crystal_F_000             2226
_exptl_absorpt_coefficient_mu    3.548
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_correction_T_min  0.4631
_exptl_absorpt_correction_T_max  0.5473
_exptl_absorpt_process_details   SADABS

_exptl_special_details           
; 
 ? 
;

_diffrn_ambient_temperature      293(2)
_diffrn_radiation_wavelength     0.71073
_diffrn_radiation_type           MoK\a
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_monochromator  graphite
_diffrn_measurement_device_type  'Bruker Smart APEX CCD area detector'
_diffrn_measurement_method       'phi and omega scans'
_diffrn_detector_area_resol_mean ?
_diffrn_standards_number         ?
_diffrn_standards_interval_count ?
_diffrn_standards_interval_time  ?
_diffrn_standards_decay_%        ?
_diffrn_reflns_number            16278
_diffrn_reflns_av_R_equivalents  0.0460
_diffrn_reflns_av_sigmaI/netI    0.0833
_diffrn_reflns_limit_h_min       -12
_diffrn_reflns_limit_h_max       12
_diffrn_reflns_limit_k_min       -15
_diffrn_reflns_limit_k_max       15
_diffrn_reflns_limit_l_min       -24
_diffrn_reflns_limit_l_max       26
_diffrn_reflns_theta_min         0.94
_diffrn_reflns_theta_max         25.15
_reflns_number_total             10394
_reflns_number_gt                7095
_reflns_threshold_expression     >2sigma(I)

_computing_data_collection       'Bruker SMART'
_computing_cell_refinement       'Bruker SMART'
_computing_data_reduction        'Bruker SAINT'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_molecular_graphics    SHELXP-97
_computing_publication_material  SHELXTL

_refine_special_details          
; 
 Refinement of F² against ALL reflections.  The weighted R-factor wR and 
 goodness of fit S are based on F², conventional R-factors R are based 
 on F, with F set to zero for negative F². The threshold expression of 
 F² > 2sigma(F²) is used only for calculating R-factors(gt) etc. and is 
 not relevant to the choice of reflections for refinement.  R-factors based 
 on F² are statistically about twice as large as those based on F, and R- 
 factors based on ALL data will be even larger. 
;

_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'calc w=1/[σ²(Fo²)+(0.0940P)²+46.9276P] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_atom_sites_solution_hydrogens   geom
_refine_ls_hydrogen_treatment    mixed
_refine_ls_extinction_method     SHELXL
_refine_ls_extinction_coef       0.00008(6)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_number_reflns         10394
_refine_ls_number_parameters     830
_refine_ls_number_restraints     432
_refine_ls_R_factor_all          0.1114
_refine_ls_R_factor_gt           0.0759
_refine_ls_wR_factor_ref         0.2107
_refine_ls_wR_factor_gt          0.1891
_refine_ls_goodness_of_fit_ref   1.041
_refine_ls_restrained_S_all      1.024
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
O2W O 0.956(3) 0.886(2) 0.5405(15) 0.102(11) Uani 0.50 1 d PU . .
H2WA H 0.8905 0.9163 0.5675 0.122 Uiso 1 1 d R . .
H2WB H 1.0259 0.9061 0.5352 0.122 Uiso 1 1 d R . .
As1 As 0.53432(13) 0.23597(10) 0.25234(6) 0.0187(3) Uani 1 1 d . . .
Mo1 Mo 0.86670(11) 0.09491(9) 0.19659(6) 0.0248(3) Uani 1 1 d U . .
Mo2 Mo 0.37955(11) 0.40434(9) 0.14445(5) 0.0233(3) Uani 1 1 d . . .
Mo3 Mo 0.20116(12) 0.35655(9) 0.31528(6) 0.0273(3) Uani 1 1 d . . .
Mo4 Mo 0.75761(12) 0.39942(9) 0.23530(6) 0.0263(3) Uani 1 1 d . . .
Mo5 Mo 0.29672(12) 0.08461(10) 0.28288(6) 0.0298(3) Uani 1 1 d . . .
Mo6 Mo 0.47505(12) 0.13323(9) 0.11204(5) 0.0238(3) Uani 1 1 d . . .
Mo7 Mo 0.70554(13) 0.05196(10) 0.34827(6) 0.0308(3) Uani 1 1 d . . .
Mo8 Mo 0.59443(12) 0.35864(10) 0.38492(6) 0.0281(3) Uani 1 1 d . . .
Cu2 Cu 0.19672(14) 0.25173(11) 0.18792(7) 0.0195(4) Uani 1 1 d . . .
Cu1 Cu 0.87153(15) 0.21609(13) 0.31908(7) 0.0231(4) Uani 1 1 d . . .
V1 V 0.6910(2) 0.27777(17) 0.09673(10) 0.0227(5) Uani 1 1 d . . .
V4 V 0.4447(2) 0.51103(17) 0.28608(11) 0.0250(5) Uani 1 1 d . . .
V2 V 0.6392(2) -0.04008(18) 0.22036(11) 0.0291(6) Uani 1 1 d . . .
V3 V 0.3654(2) 0.19337(19) 0.40542(11) 0.0305(6) Uani 1 1 d . . .
O1 O 0.5177(9) 0.2559(7) 0.1776(4) 0.024(2) Uani 1 1 d . . .
O2 O 0.4176(9) 0.4764(7) 0.2031(4) 0.028(2) Uani 1 1 d . . .
O3 O 0.5739(9) 0.0338(7) 0.1504(4) 0.030(2) Uani 1 1 d . . .
O4 O 0.3370(9) 0.2729(7) 0.1148(4) 0.028(2) Uani 1 1 d . . .
O5 O 0.8710(9) 0.0736(7) 0.2909(5) 0.032(2) Uani 1 1 d . . .
O6 O 0.1622(9) 0.2254(7) 0.2781(5) 0.033(2) Uani 1 1 d . . .
O7 O 0.6023(9) 0.1826(7) 0.0644(4) 0.027(2) Uani 1 1 d . . .
O8 O 0.3949(9) 0.2230(7) 0.2971(4) 0.027(2) Uani 1 1 d . . .
O9 O 0.2083(10) 0.3023(8) 0.3896(4) 0.034(2) Uani 1 1 d . . .
O10 O 1.0306(9) 0.0615(8) 0.1703(5) 0.038(3) Uani 1 1 d . . .
O11 O 0.8018(8) 0.1651(7) 0.1353(4) 0.027(2) Uani 1 1 d . . .
O12 O 0.8477(9) 0.2392(7) 0.2400(4) 0.028(2) Uani 1 1 d . . .
O13 O 0.5728(9) 0.3390(7) 0.2798(4) 0.025(2) Uani 1 1 d . . .
O14 O 0.7659(9) 0.3702(8) 0.3255(4) 0.032(2) Uani 1 1 d . . .
O15 O 0.4630(10) 0.2964(7) 0.4082(5) 0.035(2) Uani 1 1 d . . .
O16 O 0.0454(10) 0.4314(8) 0.3266(4) 0.038(3) Uani 1 1 d . . .
O17 O 0.2700(11) 0.4929(8) 0.1117(5) 0.042(3) Uani 1 1 d . . .
O18 O 0.6501(8) 0.1257(7) 0.2547(4) 0.024(2) Uani 1 1 d . . .
O19 O 0.2822(10) 0.1000(7) 0.3659(5) 0.034(2) Uani 1 1 d . . .
O20 O 0.2990(9) 0.4466(7) 0.3157(4) 0.029(2) Uani 1 1 d . . .
O21 O 0.3283(9) 0.1375(7) 0.1919(4) 0.028(2) Uani 1 1 d . . .
O22 O 0.8182(9) -0.0236(7) 0.1878(5) 0.033(2) Uani 1 1 d . . .
O23 O 0.6427(11) 0.3803(8) 0.4510(5) 0.040(3) Uani 1 1 d . . .
O24 O 0.7256(9) 0.3663(7) 0.1611(4) 0.030(2) Uani 1 1 d . . .
O25 O 0.8956(10) 0.4426(8) 0.2163(5) 0.039(3) Uani 1 1 d . . .
O26 O 0.6299(9) 0.5153(7) 0.2526(5) 0.034(2) Uani 1 1 d . . .
O27 O 0.6596(10) -0.1594(7) 0.2016(5) 0.037(3) Uani 1 1 d . . .
O28 O 0.2477(8) 0.3583(7) 0.2172(4) 0.027(2) Uani 1 1 d . . .
O29 O 0.7864(10) 0.2981(8) 0.0372(5) 0.041(3) Uani 1 1 d . . .
O30 O 0.3727(11) 0.6310(8) 0.2946(5) 0.045(3) Uani 1 1 d . . .
O31 O 0.5059(10) 0.4867(7) 0.3661(4) 0.034(2) Uani 1 1 d . . .
O32 O 0.1946(12) 0.0088(9) 0.2768(6) 0.050(3) Uani 1 1 d . . .
O33 O 0.7149(10) 0.2060(7) 0.3620(5) 0.034(2) Uani 1 1 d . . .
O34 O 0.7032(11) -0.0571(7) 0.3018(5) 0.039(3) Uani 1 1 d . . .
O35 O 0.7801(12) -0.0046(8) 0.4074(5) 0.049(3) Uani 1 1 d . . .
O36 O 0.4578(9) 0.0039(7) 0.2637(5) 0.033(2) Uani 1 1 d . . .
O37 O 0.4167(10) 0.0716(8) 0.0610(4) 0.035(2) Uani 1 1 d . . .
O38 O 0.5381(10) 0.0971(8) 0.3825(5) 0.036(2) Uani 1 1 d . . .
O39 O 0.5272(9) 0.3856(7) 0.0886(4) 0.027(2) Uani 1 1 d . . .
O40 O 0.3216(12) 0.1696(9) 0.4764(5) 0.051(3) Uani 1 1 d . . .
N3 N 0.1505(14) 0.5202(12) 0.5147(7) 0.052(4) Uani 1 1 d U . .
C1 C 0.081(2) 0.6129(18) 0.5362(10) 0.068(3) Uani 1 1 d U . .
H1 H 0.0328 0.6288 0.5760 0.082 Uiso 1 1 calc R . .
N4 N 0.0933(16) 0.6779(16) 0.4922(9) 0.075(5) Uani 1 1 d . . .
C2 C 0.176(2) 0.7972(17) 0.2064(11) 0.076(3) Uani 1 1 d U . .
H2A H 0.2381 0.7816 0.2344 0.091 Uiso 1 1 calc R . .
H2B H 0.1276 0.8686 0.2146 0.091 Uiso 1 1 calc R . .
N6 N 0.0081(15) 0.6010(12) 0.2428(8) 0.061(4) Uani 1 1 d . . .
H6A H 0.0044 0.5393 0.2529 0.073 Uiso 1 1 calc R . .
N7 N 0.5339(15) 0.7221(10) 0.0915(7) 0.050(4) Uani 1 1 d . . .
C3 C 0.111(2) 0.6390(17) 0.2412(11) 0.075(3) Uani 1 1 d U . .
H3 H 0.1887 0.6043 0.2532 0.089 Uiso 1 1 calc R . .
N1 N 0.1435(13) 0.1340(10) 0.9872(6) 0.042(3) Uani 1 1 d U . .
C4 C 0.0614(16) -0.0175(13) 1.0127(8) 0.049(3) Uani 1 1 d U . .
H4A H 0.0416 0.0015 1.0565 0.059 Uiso 1 1 calc R . .
H4B H 0.0878 -0.0923 1.0091 0.059 Uiso 1 1 calc R . .
C5 C 0.1741(17) 0.0228(13) 0.9838(8) 0.048(3) Uani 1 1 d U . .
H5A H 0.2471 -0.0045 1.0047 0.058 Uiso 1 1 calc R . .
H5B H 0.2005 -0.0007 0.9408 0.058 Uiso 1 1 calc R . .
N5 N 0.0884(14) 0.7338(11) 0.2198(8) 0.054(4) Uani 1 1 d . . .
C6 C -0.042(2) 0.7558(17) 0.2120(11) 0.075(3) Uani 1 1 d U . .
H6 H -0.0877 0.8183 0.1988 0.090 Uiso 1 1 calc R . .
C7 C 0.463(2) 0.8309(17) 0.1039(11) 0.073(3) Uani 1 1 d U . .
H7A H 0.4802 0.8547 0.1424 0.088 Uiso 1 1 calc R . .
H7B H 0.4956 0.8722 0.0710 0.088 Uiso 1 1 calc R . .
C8 C 0.288(2) 0.3859(17) 0.5746(10) 0.072(3) Uani 1 1 d U . .
H8A H 0.3584 0.3632 0.5395 0.087 Uiso 1 1 calc R . .
H8B H 0.3065 0.4423 0.5959 0.087 Uiso 1 1 calc R . .
C9 C 0.284(2) 0.2981(18) 0.6180(10) 0.075(3) Uani 1 1 d U . .
H9A H 0.2098 0.3201 0.6515 0.091 Uiso 1 1 calc R . .
H9B H 0.2694 0.2410 0.5957 0.091 Uiso 1 1 calc R . .
C10 C 0.160(2) 0.4247(17) 0.5513(10) 0.072(3) Uani 1 1 d U . .
H10A H 0.1481 0.3703 0.5258 0.086 Uiso 1 1 calc R . .
H10B H 0.0891 0.4377 0.5867 0.086 Uiso 1 1 calc R . .
C11 C 0.174(2) 0.6196(18) 0.4405(10) 0.070(4) Uani 1 1 d U . .
H11 H 0.1980 0.6451 0.4016 0.084 Uiso 1 1 calc R . .
C12 C 0.209(2) 0.5278(18) 0.4555(10) 0.068(3) Uani 1 1 d U . .
H12 H 0.2648 0.4740 0.4302 0.082 Uiso 1 1 calc R . .
C13 C -0.092(2) 0.6739(16) 0.2262(11) 0.074(4) Uani 1 1 d U . .
H13 H -0.1759 0.6681 0.2249 0.089 Uiso 1 1 calc R . .
C14 C 0.402(2) 0.2607(18) 0.6449(10) 0.076(3) Uani 1 1 d U . .
H14A H 0.4238 0.3190 0.6624 0.092 Uiso 1 1 calc R . .
H14B H 0.3836 0.2152 0.6783 0.092 Uiso 1 1 calc R . .
N9 N 0.5137(15) 0.2054(12) 0.5999(7) 0.050(4) Uani 1 1 d U . .
C16 C 0.1030(16) 0.1951(12) 1.0376(8) 0.044(3) Uani 1 1 d U . .
H16 H 0.0900 0.1717 1.0778 0.053 Uiso 1 1 calc R . .
C17 C 0.1451(18) 0.1985(14) 0.9370(9) 0.052(3) Uani 1 1 d U . .
H17 H 0.1672 0.1796 0.8951 0.062 Uiso 1 1 calc R . .
C18 C 0.0835(15) 0.2933(12) 1.0236(8) 0.039(3) Uani 1 1 d U . .
H18 H 0.0579 0.3497 1.0513 0.046 Uiso 1 1 calc R . .
N2 N 0.107(2) 0.2962(19) 0.9634(11) 0.107(7) Uani 1 1 d U . .
H2 H 0.0992 0.3520 0.9429 0.129 Uiso 1 1 calc R . .
O1W O 1.0185(12) 0.4712(9) 0.0950(5) 0.052(3) Uani 1 1 d U . .
H1WA H 0.9709 0.4783 0.1309 0.063 Uiso 1 1 d R . .
H1WB H 1.0864 0.4905 0.0967 0.063 Uiso 1 1 d R . .
N8 N 0.6338(14) 0.5638(10) 0.1084(6) 0.042(3) Uani 1 1 d U . .
C19 C 0.627(2) 0.5711(16) 0.0446(10) 0.066(4) Uani 1 1 d U . .
H19 H 0.6599 0.5193 0.0139 0.079 Uiso 1 1 calc R . .
C20 C 0.577(2) 0.6568(17) 0.1349(11) 0.072(3) Uani 1 1 d U . .
H20 H 0.5694 0.6740 0.1766 0.087 Uiso 1 1 calc R . .
C21 C 0.563(2) 0.6698(18) 0.0382(11) 0.074(3) Uani 1 1 d U . .
H21 H 0.5423 0.6973 0.0012 0.088 Uiso 1 1 calc R . .
N10 N 0.641(2) 0.0849(16) 0.5376(9) 0.085(6) Uani 1 1 d U . .
H10 H 0.6766 0.0253 0.5197 0.102 Uiso 1 1 calc R . .
C23 C 0.673(3) 0.1723(19) 0.5221(11) 0.083(4) Uani 1 1 d U . .
H23 H 0.7441 0.1792 0.4927 0.100 Uiso 1 1 calc R . .
C24 C 0.538(2) 0.108(2) 0.5884(11) 0.083(4) Uani 1 1 d U . .
H24 H 0.4959 0.0613 0.6097 0.100 Uiso 1 1 calc R . .
C25 C 0.585(2) 0.250(2) 0.5561(11) 0.081(3) Uani 1 1 d U . .
H25 H 0.5755 0.3200 0.5503 0.097 Uiso 1 1 calc R . .
C26 C 0.247(2) 0.7869(18) 0.1439(11) 0.080(3) Uani 1 1 d U . .
H26A H 0.3043 0.7179 0.1414 0.096 Uiso 1 1 calc R . .
H26B H 0.1824 0.7834 0.1191 0.096 Uiso 1 1 calc R . .
C27 C 0.326(2) 0.8462(19) 0.1081(11) 0.083(3) Uani 1 1 d U . .
H27A H 0.3120 0.8415 0.0659 0.099 Uiso 1 1 calc R . .
H27B H 0.2877 0.9175 0.1222 0.099 Uiso 1 1 calc R . .


_geom_special_details            
; 
 All esds (except the esd in the dihedral angle between two l.s. planes) 
 are estimated using the full covariance matrix.  The cell esds are taken 
 into account individually in the estimation of esds in distances, angles 
 and torsion angles; correlations between esds in cell parameters are only 
 used when they are defined by crystal symmetry.  An approximate (isotropic) 
 treatment of cell esds is used for estimating esds involving l.s. planes. 
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
O2W H2WA 0.8500 . ?
O2W H2WB 0.8501 . ?
As1 O13 1.678(9) . ?
As1 O8 1.681(9) . ?
As1 O18 1.687(8) . ?
As1 O1 1.692(9) . ?
Mo1 O10 1.698(10) . ?
Mo1 O11 1.779(9) . ?
Mo1 O22 1.805(10) . ?
Mo1 O5 2.094(10) . ?
Mo1 O12 2.109(9) . ?
Mo1 O18 2.382(9) . ?
Mo2 O17 1.705(10) . ?
Mo2 O2 1.778(9) . ?
Mo2 O39 1.785(9) . ?
Mo2 O4 2.060(9) . ?
Mo2 O28 2.125(9) . ?
Mo2 O1 2.363(9) . ?
Mo3 O16 1.702(10) . ?
Mo3 O20 1.781(10) . ?
Mo3 O9 1.784(10) . ?
Mo3 O6 2.103(10) . ?
Mo3 O28 2.121(9) . ?
Mo3 O8 2.362(9) . ?
Mo4 O25 1.699(10) . ?
Mo4 O26 1.793(10) . ?
Mo4 O24 1.807(9) . ?
Mo4 O14 2.028(10) . ?
Mo4 O12 2.133(9) . ?
Mo4 O13 2.366(9) . ?
Mo5 O32 1.685(11) . ?
Mo5 O36 1.780(9) . ?
Mo5 O19 1.811(10) . ?
Mo5 O6 2.089(10) . ?
Mo5 O21 2.108(9) . ?
Mo5 O8 2.389(9) . ?
Mo6 O37 1.689(9) . ?
Mo6 O3 1.791(9) . ?
Mo6 O7 1.817(9) . ?
Mo6 O4 2.074(9) . ?
Mo6 O21 2.125(9) . ?
Mo6 O1 2.373(9) . ?
Mo7 O35 1.718(11) . ?
Mo7 O38 1.775(10) . ?
Mo7 O34 1.797(10) . ?
Mo7 O5 2.063(10) . ?
Mo7 O33 2.112(10) . ?
Mo7 O18 2.377(9) . ?
Mo8 O23 1.677(10) . ?
Mo8 O15 1.800(10) . ?
Mo8 O31 1.826(10) . ?
Mo8 O14 2.092(10) . ?
Mo8 O33 2.143(10) . ?
Mo8 O13 2.385(9) . ?
Cu2 O28 1.808(9) . ?
Cu2 O21 1.823(9) . ?
Cu2 O6 1.991(10) . ?
Cu2 O4 2.060(9) . ?
Cu1 O33 1.807(10) . ?
Cu1 O12 1.812(9) . ?
Cu1 O5 2.011(10) . ?
Cu1 O14 2.087(10) . ?
V1 O29 1.573(10) . ?
V1 O11 1.964(9) . ?
V1 O7 1.971(10) . ?
V1 O24 1.993(10) . ?
V1 O39 2.018(9) . ?
V1 O1 2.400(9) . ?
V4 O30 1.598(10) . ?
V4 O20 1.970(10) . ?
V4 O2 1.974(10) . ?
V4 O31 1.980(10) . ?
V4 O26 2.005(10) . ?
V4 O13 2.365(9) . ?
V2 O27 1.604(10) . ?
V2 O36 1.956(10) . ?
V2 O3 1.959(10) . ?
V2 O22 1.989(10) . ?
V2 O34 2.019(11) . ?
V2 O18 2.385(9) . ?
V3 O40 1.596(11) . ?
V3 O15 1.930(11) . ?
V3 O38 1.965(10) . ?
V3 O19 1.989(10) . ?
V3 O9 2.021(10) . ?
V3 O8 2.384(9) . ?
N3 C1 1.32(2) . ?
N3 C12 1.35(2) . ?
N3 C10 1.49(3) . ?
C1 N4 1.30(3) . ?
C1 H1 0.9300 . ?
N4 C11 1.41(3) . ?
C2 N5 1.41(2) . ?
C2 C26 1.44(3) . ?
C2 H2A 0.9700 . ?
C2 H2B 0.9700 . ?
N6 C3 1.32(3) . ?
N6 C13 1.36(2) . ?
N6 H6A 0.8600 . ?
N7 C21 1.32(3) . ?
N7 C20 1.35(2) . ?
N7 C7 1.47(2) . ?
C3 N5 1.33(2) . ?
C3 H3 0.9300 . ?
N1 C16 1.32(2) . ?
N1 C17 1.39(2) . ?
N1 C5 1.44(2) . ?
C4 C5 1.48(2) . ?
C4 C4 1.49(3) 2_557 ?
C4 H4A 0.9700 . ?
C4 H4B 0.9700 . ?
C5 H5A 0.9700 . ?
C5 H5B 0.9700 . ?
N5 C6 1.40(3) . ?
C6 C13 1.34(3) . ?
C6 H6 0.9300 . ?
C7 C27 1.42(3) . ?
C7 H7A 0.9700 . ?
C7 H7B 0.9700 . ?
C8 C9 1.51(3) . ?
C8 C10 1.52(3) . ?
C8 H8A 0.9700 . ?
C8 H8B 0.9700 . ?
C9 C14 1.47(3) . ?
C9 H9A 0.9700 . ?
C9 H9B 0.9700 . ?
C10 H10A 0.9700 . ?
C10 H10B 0.9700 . ?
C11 C12 1.25(3) . ?
C11 H11 0.9300 . ?
C12 H12 0.9300 . ?
C13 H13 0.9300 . ?
C14 N9 1.45(2) . ?
C14 H14A 0.9700 . ?
C14 H14B 0.9700 . ?
N9 C24 1.29(3) . ?
N9 C25 1.34(3) . ?
C16 C18 1.32(2) . ?
C16 H16 0.9300 . ?
C17 N2 1.37(3) . ?
C17 H17 0.9300 . ?
C18 N2 1.30(3) . ?
C18 H18 0.9300 . ?
N2 H2 0.8600 . ?
O1W H1WA 0.8504 . ?
O1W H1WB 0.8365 . ?
N8 C20 1.33(2) . ?
N8 C19 1.41(2) . ?
C19 C21 1.35(3) . ?
C19 H19 0.9300 . ?
C20 H20 0.9300 . ?
C21 H21 0.9300 . ?
N10 C23 1.32(3) . ?
N10 C24 1.40(3) . ?
N10 H10 0.8600 . ?
C23 C25 1.34(3) . ?
C23 H23 0.9300 . ?
C24 H24 0.9300 . ?
C25 H25 0.9300 . ?
C26 C27 1.42(3) . ?
C26 H26A 0.9700 . ?
C26 H26B 0.9700 . ?
C27 H27A 0.9700 . ?
C27 H27B 0.9700 . ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
H2WA O2W H2WB 120.0 . . ?
O13 As1 O8 107.8(5) . . ?
O13 As1 O18 112.5(4) . . ?
O8 As1 O18 108.1(5) . . ?
O13 As1 O1 108.4(4) . . ?
O8 As1 O1 111.9(4) . . ?
O18 As1 O1 108.3(4) . . ?
O10 Mo1 O11 104.3(5) . . ?
O10 Mo1 O22 103.5(5) . . ?
O11 Mo1 O22 99.6(4) . . ?
O10 Mo1 O5 97.6(5) . . ?
O11 Mo1 O5 151.4(4) . . ?
O22 Mo1 O5 92.9(4) . . ?
O10 Mo1 O12 99.9(4) . . ?
O11 Mo1 O12 86.9(4) . . ?
O22 Mo1 O12 153.2(4) . . ?
O5 Mo1 O12 71.2(4) . . ?
O10 Mo1 O18 167.0(4) . . ?
O11 Mo1 O18 88.6(4) . . ?
O22 Mo1 O18 75.3(4) . . ?
O5 Mo1 O18 69.7(3) . . ?
O12 Mo1 O18 79.0(3) . . ?
O17 Mo2 O2 104.1(5) . . ?
O17 Mo2 O39 103.5(5) . . ?
O2 Mo2 O39 100.2(4) . . ?
O17 Mo2 O4 98.2(5) . . ?
O2 Mo2 O4 150.5(4) . . ?
O39 Mo2 O4 93.0(4) . . ?
O17 Mo2 O28 99.1(4) . . ?
O2 Mo2 O28 85.6(4) . . ?
O39 Mo2 O28 154.4(4) . . ?
O4 Mo2 O28 71.8(4) . . ?
O17 Mo2 O1 167.8(4) . . ?
O2 Mo2 O1 87.8(4) . . ?
O39 Mo2 O1 76.2(4) . . ?
O4 Mo2 O1 69.8(3) . . ?
O28 Mo2 O1 79.2(3) . . ?
O16 Mo3 O20 104.1(5) . . ?
O16 Mo3 O9 101.5(5) . . ?
O20 Mo3 O9 101.0(5) . . ?
O16 Mo3 O6 96.9(5) . . ?
O20 Mo3 O6 151.6(4) . . ?
O9 Mo3 O6 93.3(4) . . ?
O16 Mo3 O28 99.4(4) . . ?
O20 Mo3 O28 86.3(4) . . ?
O9 Mo3 O28 155.4(4) . . ?
O6 Mo3 O28 71.4(4) . . ?
O16 Mo3 O8 167.4(4) . . ?
O20 Mo3 O8 88.5(4) . . ?
O9 Mo3 O8 76.6(4) . . ?
O6 Mo3 O8 70.9(3) . . ?
O28 Mo3 O8 80.2(3) . . ?
O25 Mo4 O26 103.9(5) . . ?
O25 Mo4 O24 103.5(5) . . ?
O26 Mo4 O24 98.3(4) . . ?
O25 Mo4 O14 98.4(5) . . ?
O26 Mo4 O14 94.1(4) . . ?
O24 Mo4 O14 151.3(4) . . ?
O25 Mo4 O12 98.2(4) . . ?
O26 Mo4 O12 155.8(4) . . ?
O24 Mo4 O12 85.9(4) . . ?
O14 Mo4 O12 72.8(4) . . ?
O25 Mo4 O13 169.9(4) . . ?
O26 Mo4 O13 76.4(4) . . ?
O24 Mo4 O13 86.4(4) . . ?
O14 Mo4 O13 71.5(3) . . ?
O12 Mo4 O13 80.1(3) . . ?
O32 Mo5 O36 106.2(5) . . ?
O32 Mo5 O19 102.8(5) . . ?
O36 Mo5 O19 100.2(4) . . ?
O32 Mo5 O6 96.5(5) . . ?
O36 Mo5 O6 150.7(4) . . ?
O19 Mo5 O6 92.3(4) . . ?
O32 Mo5 O21 101.1(5) . . ?
O36 Mo5 O21 86.3(4) . . ?
O19 Mo5 O21 152.3(4) . . ?
O6 Mo5 O21 71.1(4) . . ?
O32 Mo5 O8 166.5(5) . . ?
O36 Mo5 O8 87.3(4) . . ?
O19 Mo5 O8 74.7(4) . . ?
O6 Mo5 O8 70.6(4) . . ?
O21 Mo5 O8 78.9(3) . . ?
O37 Mo6 O3 105.8(5) . . ?
O37 Mo6 O7 104.3(5) . . ?
O3 Mo6 O7 99.7(4) . . ?
O37 Mo6 O4 96.5(4) . . ?
O3 Mo6 O4 150.5(4) . . ?
O7 Mo6 O4 93.1(4) . . ?
O37 Mo6 O21 99.8(4) . . ?
O3 Mo6 O21 85.1(4) . . ?
O7 Mo6 O21 152.9(4) . . ?
O4 Mo6 O21 72.0(4) . . ?
O37 Mo6 O1 165.7(4) . . ?
O3 Mo6 O1 88.2(4) . . ?
O7 Mo6 O1 75.5(4) . . ?
O4 Mo6 O1 69.3(3) . . ?
O21 Mo6 O1 78.0(3) . . ?
O35 Mo7 O38 104.8(5) . . ?
O35 Mo7 O34 102.9(5) . . ?
O38 Mo7 O34 102.0(5) . . ?
O35 Mo7 O5 97.3(5) . . ?
O38 Mo7 O5 150.4(4) . . ?
O34 Mo7 O5 91.8(4) . . ?
O35 Mo7 O33 99.6(5) . . ?
O38 Mo7 O33 84.8(4) . . ?
O34 Mo7 O33 153.9(4) . . ?
O5 Mo7 O33 72.2(4) . . ?
O35 Mo7 O18 167.4(5) . . ?
O38 Mo7 O18 87.6(4) . . ?
O34 Mo7 O18 76.1(4) . . ?
O5 Mo7 O18 70.3(3) . . ?
O33 Mo7 O18 79.0(3) . . ?
O23 Mo8 O15 104.7(5) . . ?
O23 Mo8 O31 103.4(5) . . ?
O15 Mo8 O31 101.5(4) . . ?
O23 Mo8 O14 96.3(5) . . ?
O15 Mo8 O14 151.2(4) . . ?
O31 Mo8 O14 92.3(4) . . ?
O23 Mo8 O33 99.0(5) . . ?
O15 Mo8 O33 85.6(4) . . ?
O31 Mo8 O33 153.8(4) . . ?
O14 Mo8 O33 71.6(4) . . ?
O23 Mo8 O13 166.2(4) . . ?
O15 Mo8 O13 88.8(4) . . ?
O31 Mo8 O13 76.0(4) . . ?
O14 Mo8 O13 70.1(3) . . ?
O33 Mo8 O13 79.0(3) . . ?
O28 Cu2 O21 105.8(4) . . ?
O28 Cu2 O6 80.7(4) . . ?
O21 Cu2 O6 79.4(4) . . ?
O28 Cu2 O4 78.5(4) . . ?
O21 Cu2 O4 78.7(4) . . ?
O6 Cu2 O4 144.3(4) . . ?
O33 Cu1 O12 105.5(4) . . ?
O33 Cu1 O5 80.0(4) . . ?
O12 Cu1 O5 79.3(4) . . ?
O33 Cu1 O14 78.7(4) . . ?
O12 Cu1 O14 78.2(4) . . ?
O5 Cu1 O14 143.5(4) . . ?
O29 V1 O11 103.0(5) . . ?
O29 V1 O7 102.3(5) . . ?
O11 V1 O7 92.0(4) . . ?
O29 V1 O24 102.3(5) . . ?
O11 V1 O24 84.0(4) . . ?
O7 V1 O24 155.4(4) . . ?
O29 V1 O39 100.4(5) . . ?
O11 V1 O39 156.6(4) . . ?
O7 V1 O39 83.9(4) . . ?
O24 V1 O39 90.2(4) . . ?
O29 V1 O1 170.5(5) . . ?
O11 V1 O1 85.2(3) . . ?
O7 V1 O1 72.3(3) . . ?
O24 V1 O1 83.1(4) . . ?
O39 V1 O1 71.5(3) . . ?
O30 V4 O20 101.6(5) . . ?
O30 V4 O2 102.3(5) . . ?
O20 V4 O2 84.1(4) . . ?
O30 V4 O31 100.4(5) . . ?
O20 V4 O31 90.9(4) . . ?
O2 V4 O31 157.2(4) . . ?
O30 V4 O26 101.9(5) . . ?
O20 V4 O26 156.5(4) . . ?
O2 V4 O26 91.5(4) . . ?
O31 V4 O26 84.3(4) . . ?
O30 V4 O13 172.4(5) . . ?
O20 V4 O13 83.7(4) . . ?
O2 V4 O13 83.5(4) . . ?
O31 V4 O13 73.9(4) . . ?
O26 V4 O13 72.9(4) . . ?
O27 V2 O36 104.9(5) . . ?
O27 V2 O3 103.9(5) . . ?
O36 V2 O3 85.0(4) . . ?
O27 V2 O22 99.5(5) . . ?
O36 V2 O22 155.5(4) . . ?
O3 V2 O22 90.9(4) . . ?
O27 V2 O34 99.2(5) . . ?
O36 V2 O34 90.9(4) . . ?
O3 V2 O34 156.9(4) . . ?
O22 V2 O34 83.4(4) . . ?
O27 V2 O18 168.5(4) . . ?
O36 V2 O18 83.3(4) . . ?
O3 V2 O18 84.6(4) . . ?
O22 V2 O18 72.2(3) . . ?
O34 V2 O18 72.3(4) . . ?
O40 V3 O15 104.3(5) . . ?
O40 V3 O38 102.9(6) . . ?
O15 V3 O38 84.7(4) . . ?
O40 V3 O19 99.4(5) . . ?
O15 V3 O19 156.3(4) . . ?
O38 V3 O19 91.3(4) . . ?
O40 V3 O9 101.9(5) . . ?
O15 V3 O9 91.0(4) . . ?
O38 V3 O9 155.2(4) . . ?
O19 V3 O9 82.9(4) . . ?
O40 V3 O8 169.8(5) . . ?
O15 V3 O8 84.4(4) . . ?
O38 V3 O8 83.1(4) . . ?
O19 V3 O8 71.9(4) . . ?
O9 V3 O8 72.1(4) . . ?
As1 O1 Mo2 123.8(4) . . ?
As1 O1 Mo6 124.2(5) . . ?
Mo2 O1 Mo6 97.4(3) . . ?
As1 O1 V1 123.8(5) . . ?
Mo2 O1 V1 89.1(3) . . ?
Mo6 O1 V1 88.5(3) . . ?
Mo2 O2 V4 158.0(6) . . ?
Mo6 O3 V2 157.1(5) . . ?
Mo2 O4 Cu2 101.2(4) . . ?
Mo2 O4 Mo6 118.8(5) . . ?
Cu2 O4 Mo6 100.9(4) . . ?
Cu1 O5 Mo7 100.8(4) . . ?
Cu1 O5 Mo1 101.1(4) . . ?
Mo7 O5 Mo1 118.5(5) . . ?
Cu2 O6 Mo5 101.7(4) . . ?
Cu2 O6 Mo3 100.8(4) . . ?
Mo5 O6 Mo3 116.8(5) . . ?
Mo6 O7 V1 123.2(5) . . ?
As1 O8 Mo3 123.2(5) . . ?
As1 O8 V3 125.5(5) . . ?
Mo3 O8 V3 89.0(3) . . ?
As1 O8 Mo5 123.0(5) . . ?
Mo3 O8 Mo5 97.4(3) . . ?
V3 O8 Mo5 89.2(3) . . ?
Mo3 O9 V3 121.7(5) . . ?
Mo1 O11 V1 156.9(6) . . ?
Cu1 O12 Mo1 107.7(4) . . ?
Cu1 O12 Mo4 107.2(4) . . ?
Mo1 O12 Mo4 141.6(5) . . ?
As1 O13 V4 125.9(5) . . ?
As1 O13 Mo4 124.0(5) . . ?
V4 O13 Mo4 89.0(3) . . ?
As1 O13 Mo8 123.2(5) . . ?
V4 O13 Mo8 88.5(3) . . ?
Mo4 O13 Mo8 96.1(3) . . ?
Mo4 O14 Cu1 101.3(4) . . ?
Mo4 O14 Mo8 118.2(4) . . ?
Cu1 O14 Mo8 100.4(4) . . ?
Mo8 O15 V3 156.5(6) . . ?
As1 O18 Mo7 123.5(5) . . ?
As1 O18 Mo1 123.7(5) . . ?
Mo7 O18 Mo1 97.3(3) . . ?
As1 O18 V2 124.7(4) . . ?
Mo7 O18 V2 89.0(3) . . ?
Mo1 O18 V2 88.9(3) . . ?
Mo5 O19 V3 123.6(5) . . ?
Mo3 O20 V4 156.6(5) . . ?
Cu2 O21 Mo5 107.0(4) . . ?
Cu2 O21 Mo6 107.5(4) . . ?
Mo5 O21 Mo6 142.9(5) . . ?
Mo1 O22 V2 123.2(5) . . ?
Mo4 O24 V1 157.2(6) . . ?
Mo4 O26 V4 121.5(5) . . ?
Cu2 O28 Mo3 106.6(4) . . ?
Cu2 O28 Mo2 107.9(4) . . ?
Mo3 O28 Mo2 141.6(5) . . ?
Mo8 O31 V4 121.1(5) . . ?
Cu1 O33 Mo7 106.2(5) . . ?
Cu1 O33 Mo8 108.5(5) . . ?
Mo7 O33 Mo8 142.3(5) . . ?
Mo7 O34 V2 121.9(5) . . ?
Mo5 O36 V2 157.2(6) . . ?
Mo7 O38 V3 158.7(6) . . ?
Mo2 O39 V1 122.7(5) . . ?
C1 N3 C12 108.7(19) . . ?
C1 N3 C10 124.2(17) . . ?
C12 N3 C10 127.0(18) . . ?
N4 C1 N3 108(2) . . ?
N4 C1 H1 125.9 . . ?
N3 C1 H1 125.9 . . ?
C1 N4 C11 106(2) . . ?
N5 C2 C26 115(2) . . ?
N5 C2 H2A 108.5 . . ?
C26 C2 H2A 108.5 . . ?
N5 C2 H2B 108.5 . . ?
C26 C2 H2B 108.5 . . ?
H2A C2 H2B 107.5 . . ?
C3 N6 C13 110.1(18) . . ?
C3 N6 H6A 125.0 . . ?
C13 N6 H6A 125.0 . . ?
C21 N7 C20 107.8(17) . . ?
C21 N7 C7 127.5(18) . . ?
C20 N7 C7 124.7(18) . . ?
N6 C3 N5 110.2(19) . . ?
N6 C3 H3 124.9 . . ?
N5 C3 H3 124.9 . . ?
C16 N1 C17 106.4(14) . . ?
C16 N1 C5 127.6(15) . . ?
C17 N1 C5 125.9(14) . . ?
C5 C4 C4 117(2) . 2_557 ?
C5 C4 H4A 108.0 . . ?
C4 C4 H4A 108.0 2_557 . ?
C5 C4 H4B 108.0 . . ?
C4 C4 H4B 108.0 2_557 . ?
H4A C4 H4B 107.3 . . ?
N1 C5 C4 111.8(14) . . ?
N1 C5 H5A 109.3 . . ?
C4 C5 H5A 109.3 . . ?
N1 C5 H5B 109.3 . . ?
C4 C5 H5B 109.3 . . ?
H5A C5 H5B 107.9 . . ?
C3 N5 C6 104.7(18) . . ?
C3 N5 C2 127.9(18) . . ?
C6 N5 C2 127.4(17) . . ?
C13 C6 N5 110(2) . . ?
C13 C6 H6 124.9 . . ?
N5 C6 H6 124.9 . . ?
C27 C7 N7 112.5(19) . . ?
C27 C7 H7A 109.1 . . ?
N7 C7 H7A 109.1 . . ?
C27 C7 H7B 109.1 . . ?
N7 C7 H7B 109.1 . . ?
H7A C7 H7B 107.8 . . ?
C9 C8 C10 112.2(19) . . ?
C9 C8 H8A 109.2 . . ?
C10 C8 H8A 109.2 . . ?
C9 C8 H8B 109.2 . . ?
C10 C8 H8B 109.2 . . ?
H8A C8 H8B 107.9 . . ?
C14 C9 C8 115(2) . . ?
C14 C9 H9A 108.5 . . ?
C8 C9 H9A 108.5 . . ?
C14 C9 H9B 108.5 . . ?
C8 C9 H9B 108.5 . . ?
H9A C9 H9B 107.5 . . ?
N3 C10 C8 115.3(17) . . ?
N3 C10 H10A 108.4 . . ?
C8 C10 H10A 108.4 . . ?
N3 C10 H10B 108.4 . . ?
C8 C10 H10B 108.4 . . ?
H10A C10 H10B 107.5 . . ?
C12 C11 N4 109(2) . . ?
C12 C11 H11 125.7 . . ?
N4 C11 H11 125.7 . . ?
C11 C12 N3 108(2) . . ?
C11 C12 H12 125.9 . . ?
N3 C12 H12 125.9 . . ?
C6 C13 N6 105(2) . . ?
C6 C13 H13 127.6 . . ?
N6 C13 H13 127.6 . . ?
N9 C14 C9 113.1(19) . . ?
N9 C14 H14A 109.0 . . ?
C9 C14 H14A 109.0 . . ?
N9 C14 H14B 109.0 . . ?
C9 C14 H14B 109.0 . . ?
H14A C14 H14B 107.8 . . ?
C24 N9 C25 110.2(19) . . ?
C24 N9 C14 123.0(19) . . ?
C25 N9 C14 125.1(18) . . ?
C18 C16 N1 111.4(16) . . ?
C18 C16 H16 124.3 . . ?
N1 C16 H16 124.3 . . ?
N2 C17 N1 104.3(17) . . ?
N2 C17 H17 127.9 . . ?
N1 C17 H17 127.9 . . ?
N2 C18 C16 106.9(17) . . ?
N2 C18 H18 126.5 . . ?
C16 C18 H18 126.5 . . ?
C18 N2 C17 111(2) . . ?
C18 N2 H2 124.5 . . ?
C17 N2 H2 124.5 . . ?
H1WA O1W H1WB 108.9 . . ?
C20 N8 C19 107.4(16) . . ?
C21 C19 N8 104.8(19) . . ?
C21 C19 H19 127.6 . . ?
N8 C19 H19 127.6 . . ?
N8 C20 N7 109.0(18) . . ?
N8 C20 H20 125.5 . . ?
N7 C20 H20 125.5 . . ?
N7 C21 C19 111(2) . . ?
N7 C21 H21 124.5 . . ?
C19 C21 H21 124.5 . . ?
C23 N10 C24 107(2) . . ?
C23 N10 H10 126.6 . . ?
C24 N10 H10 126.6 . . ?
N10 C23 C25 108(2) . . ?
N10 C23 H23 125.8 . . ?
C25 C23 H23 125.8 . . ?
N9 C24 N10 107(2) . . ?
N9 C24 H24 126.6 . . ?
N10 C24 H24 126.6 . . ?
N9 C25 C23 106(2) . . ?
N9 C25 H25 126.8 . . ?
C23 C25 H25 126.8 . . ?
C27 C26 C2 133(2) . . ?
C27 C26 H26A 103.9 . . ?
C2 C26 H26A 103.9 . . ?
C27 C26 H26B 103.9 . . ?
C2 C26 H26B 103.9 . . ?
H26A C26 H26B 105.4 . . ?
C7 C27 C26 125(2) . . ?
C7 C27 H27A 106.0 . . ?
C26 C27 H27A 106.0 . . ?
C7 C27 H27B 106.0 . . ?
C26 C27 H27B 106.0 . . ?
H27A C27 H27B 106.3 . . ?

loop_
_geom_hbond_atom_site_label_D
_geom_hbond_atom_site_label_H
_geom_hbond_atom_site_label_A
_geom_hbond_distance_DH
_geom_hbond_distance_HA
_geom_hbond_distance_DA
_geom_hbond_angle_DHA
_geom_hbond_site_symmetry_A
N6 H6A O16 0.86 2.19 2.898(19) 140.1 .
N6 H6A O25 0.86 2.19 2.793(19) 127.5 1_455
N2 H2 O1W 0.86 2.60 3.41(3) 157.0 2_666
O1W H1WA O25 0.85 2.01 2.817(16) 159.4 .
O1W H1WB O17 0.84 2.06 2.871(16) 162.2 1_655
N10 H10 O35 0.86 2.51 3.08(2) 124.8 .
N10 H10 O40 0.86 2.60 3.34(2) 144.5 2_656
O2W H2WA O19 0.85 2.20 2.94(3) 146.1 2_666

_diffrn_measured_fraction_theta_max 0.968
_diffrn_reflns_theta_full        25.15
_diffrn_measured_fraction_theta_full 0.968
_refine_diff_density_max         3.341
_refine_diff_density_min         -1.972
_refine_diff_density_rms         0.251


####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_3
_database_code_depnum_ccdc_archive 'CCDC 1835437'
_audit_update_record             
;
2018-05-09 deposited with the CCDC.
2018-05-21 downloaded from the CCDC.
;

_audit_creation_method           SHELXL-97
_chemical_name_systematic        
; 
 ? 
;
_chemical_name_common            ?
_chemical_melting_point          ?
_chemical_formula_moiety         'C30 H30 As Cu5 Mo12 N20 O42 V2'
_chemical_formula_sum            'C30 H30 As Cu5 Mo12 N20 O42 V2'
_chemical_formula_weight         2988.57

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
As As 0.0499 2.0058 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cu Cu 0.3201 1.2651 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
V V 0.3005 0.5294 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_H-M   'C 2/c'
_symmetry_space_group_name_Hall  '-C 2yc'
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, y, -z+1/2'
'x+1/2, y+1/2, z'
'-x+1/2, y+1/2, -z+1/2'
'-x, -y, -z'
'x, -y, z-1/2'
'-x+1/2, -y+1/2, -z'
'x+1/2, -y+1/2, z-1/2'

_cell_length_a                   20.7262(6)
_cell_length_b                   14.6357(6)
_cell_length_c                   25.6626(9)
_cell_angle_alpha                90.00
_cell_angle_beta                 113.289(2)
_cell_angle_gamma                90.00
_cell_volume                     7150.3(4)
_cell_formula_units_Z            4
_cell_measurement_temperature    293(2)
_cell_measurement_reflns_used    6345
_cell_measurement_theta_min      1.73
_cell_measurement_theta_max      25.08

_exptl_crystal_description       block
_exptl_crystal_colour            blue
_exptl_crystal_size_max          0.20
_exptl_crystal_size_mid          0.18
_exptl_crystal_size_min          0.16
_exptl_crystal_density_meas      ?
_exptl_crystal_density_diffrn    2.776
_exptl_crystal_density_method    'not measured'
_exptl_crystal_F_000             5656
_exptl_absorpt_coefficient_mu    4.287
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_correction_T_min  0.405
_exptl_absorpt_correction_T_max  0.501
_exptl_absorpt_process_details   SADABS

_exptl_special_details           
; 
 ? 
;

_diffrn_ambient_temperature      293(2)
_diffrn_radiation_wavelength     0.71073
_diffrn_radiation_type           MoK\a
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_monochromator  graphite
_diffrn_measurement_device_type  'Bruker Smart APEX CCD area detector'
_diffrn_measurement_method       'phi and omega scans'
_diffrn_detector_area_resol_mean ?
_diffrn_standards_number         ?
_diffrn_standards_interval_count ?
_diffrn_standards_interval_time  ?
_diffrn_standards_decay_%        ?
_diffrn_reflns_number            22949
_diffrn_reflns_av_R_equivalents  0.0457
_diffrn_reflns_av_sigmaI/netI    0.0430
_diffrn_reflns_limit_h_min       -24
_diffrn_reflns_limit_h_max       24
_diffrn_reflns_limit_k_min       -17
_diffrn_reflns_limit_k_max       16
_diffrn_reflns_limit_l_min       -30
_diffrn_reflns_limit_l_max       25
_diffrn_reflns_theta_min         1.73
_diffrn_reflns_theta_max         25.08
_reflns_number_total             6345
_reflns_number_gt                4944
_reflns_threshold_expression     >2sigma(I)

_computing_data_collection       'Bruker SMART'
_computing_cell_refinement       'Bruker SMART'
_computing_data_reduction        'Bruker SAINT'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_molecular_graphics    SHELXP-97
_computing_publication_material  SHELXTL

_refine_special_details          
; 
 Refinement of F² against ALL reflections.  The weighted R-factor wR and 
 goodness of fit S are based on F², conventional R-factors R are based 
 on F, with F set to zero for negative F². The threshold expression of 
 F² > 2sigma(F²) is used only for calculating R-factors(gt) etc. and is 
 not relevant to the choice of reflections for refinement.  R-factors based 
 on F² are statistically about twice as large as those based on F, and R- 
 factors based on ALL data will be even larger. 
;

_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'calc w=1/[σ²(Fo²)+(0.0610P)²+174.2442P] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_atom_sites_solution_hydrogens   geom
_refine_ls_hydrogen_treatment    mixed
_refine_ls_extinction_method     none
_refine_ls_extinction_coef       ?
_refine_ls_number_reflns         6345
_refine_ls_number_parameters     509
_refine_ls_number_restraints     18
_refine_ls_R_factor_all          0.0639
_refine_ls_R_factor_gt           0.0484
_refine_ls_wR_factor_ref         0.1451
_refine_ls_wR_factor_gt          0.1351
_refine_ls_goodness_of_fit_ref   1.050
_refine_ls_restrained_S_all      1.052
_refine_ls_shift/su_max          0.004
_refine_ls_shift/su_mean         0.000

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
As1 As 0.5000 0.32037(9) 0.2500 0.0214(3) Uani 1 2 d S . .
C1 C 0.5643(6) 0.3069(7) 0.4916(5) 0.041(3) Uani 1 1 d . . .
H1 H 0.5655 0.3347 0.4594 0.049 Uiso 1 1 calc R . .
C2 C 0.5899(8) 0.2191(11) 0.5664(6) 0.081(5) Uani 1 1 d . . .
H2 H 0.6115 0.1768 0.5951 0.097 Uiso 1 1 calc R . .
C3 C 0.5341(8) 0.2697(11) 0.5592(6) 0.078(5) Uani 1 1 d . . .
H3 H 0.5092 0.2675 0.5825 0.093 Uiso 1 1 calc R . .
C4 C 0.3439(7) 0.5347(9) 0.4121(5) 0.058(4) Uani 1 1 d . . .
H4 H 0.3654 0.5328 0.3865 0.069 Uiso 1 1 calc R . .
C5 C 0.3213(6) 0.5111(9) 0.4844(5) 0.053(3) Uani 1 1 d . . .
H5 H 0.3239 0.4898 0.5193 0.063 Uiso 1 1 calc R . .
C6 C 0.2737(7) 0.5707(10) 0.4506(6) 0.068(4) Uani 1 1 d . . .
H6 H 0.2372 0.5968 0.4579 0.081 Uiso 1 1 calc R . .
C7 C 0.6534(10) 0.7546(15) 0.3910(11) 0.142(7) Uani 1 1 d U . .
H7 H 0.6370 0.7012 0.4012 0.171 Uiso 1 1 calc R . .
N5 N 0.7226(8) 0.8477(12) 0.3817(8) 0.110(5) Uani 1 1 d . . .
C9 C 0.6557(9) 0.8696(16) 0.3514(9) 0.111(7) Uani 1 1 d . . .
H9 H 0.6422 0.9194 0.3269 0.133 Uiso 1 1 calc R . .
C10 C 0.3700(7) 0.7560(11) 0.2909(6) 0.065(4) Uani 1 1 d . . .
H10 H 0.3803 0.6945 0.2895 0.077 Uiso 1 1 calc R . .
C11 C 0.3802(9) 0.9010(11) 0.3009(8) 0.083(5) Uani 1 1 d . . .
H11 H 0.3996 0.9593 0.3085 0.100 Uiso 1 1 calc R . .
N8 N 0.3124(8) 0.8821(13) 0.2829(9) 0.124(7) Uani 1 1 d . . .
C13 C 0.1143(8) 0.5785(14) 0.0914(9) 0.110(8) Uani 1 1 d . . .
H13 H 0.0855 0.6051 0.1072 0.132 Uiso 1 1 calc R . .
N9 N 0.1847(6) 0.5796(10) 0.1156(6) 0.089(5) Uani 1 1 d . . .
C15 C 0.1508(9) 0.5135(13) 0.0374(8) 0.093(6) Uani 1 1 d . . .
H15 H 0.1523 0.4844 0.0057 0.112 Uiso 1 1 calc R . .
V1 V 0.5000 0.04348(14) 0.2500 0.0217(5) Uani 1 2 d S . .
V2 V 0.5000 0.59787(13) 0.2500 0.0155(4) Uani 1 2 d S . .
Cu1 Cu 0.44388(9) 0.40983(11) 0.48625(7) 0.0581(5) Uani 1 1 d . . .
Cu2 Cu 0.51395(9) 0.82056(13) 0.32453(9) 0.0703(5) Uani 1 1 d . . .
Cu3 Cu 0.0000 0.5000 0.0000 0.1025(12) Uani 1 2 d S . .
Mo1 Mo 0.45792(4) 0.15389(5) 0.13791(3) 0.0229(2) Uani 1 1 d . . .
Mo2 Mo 0.36464(4) 0.15465(5) 0.22895(3) 0.02230(19) Uani 1 1 d . . .
Mo3 Mo 0.33499(5) 0.31379(6) 0.12555(4) 0.0322(2) Uani 1 1 d . . .
Mo4 Mo 0.36741(4) 0.48623(5) 0.23821(3) 0.02109(19) Uani 1 1 d . . .
Mo5 Mo 0.40497(5) 0.32738(6) 0.34144(4) 0.0342(2) Uani 1 1 d . . .
Mo6 Mo 0.52930(4) 0.48692(5) 0.36013(3) 0.02080(19) Uani 1 1 d . . .
N1 N 0.6097(6) 0.2422(8) 0.5223(4) 0.056(3) Uani 1 1 d . . .
N2 N 0.5180(5) 0.3254(7) 0.5133(4) 0.054(3) Uani 1 1 d . . .
N3 N 0.3652(5) 0.4874(6) 0.4588(4) 0.048(2) Uani 1 1 d . . .
N4 N 0.2879(6) 0.5858(7) 0.4049(4) 0.059(3) Uani 1 1 d . . .
C8 C 0.7196(10) 0.7738(15) 0.4076(11) 0.133(7) Uani 1 1 d U . .
H8 H 0.7572 0.7408 0.4330 0.160 Uiso 1 1 calc R . .
N6 N 0.6127(6) 0.8165(9) 0.3592(7) 0.085(4) Uani 1 1 d U . .
N7 N 0.4155(5) 0.8260(7) 0.3062(5) 0.052(3) Uani 1 1 d . . .
C12 C 0.3036(8) 0.7951(14) 0.2773(7) 0.099(7) Uani 1 1 d . . .
H12 H 0.2611 0.7640 0.2664 0.119 Uiso 1 1 calc R . .
C14 C 0.2062(8) 0.5379(12) 0.0821(7) 0.086(5) Uani 1 1 d . . .
H14 H 0.2528 0.5266 0.0882 0.103 Uiso 1 1 calc R . .
N10 N 0.0918(6) 0.5363(9) 0.0438(5) 0.073(4) Uani 1 1 d . . .
O1 O 0.5000 -0.0655(7) 0.2500 0.043(3) Uani 1 2 d S . .
O2 O 0.4139(3) 0.0861(4) 0.1852(3) 0.0252(14) Uani 1 1 d . . .
O3 O 0.5426(3) 0.1118(4) 0.2087(3) 0.0243(13) Uani 1 1 d . . .
O4 O 0.4584(4) 0.0709(5) 0.0926(3) 0.0353(16) Uani 1 1 d . . .
O5 O 0.5173(3) 0.2412(4) 0.1315(2) 0.0258(14) Uani 1 1 d . . .
O6 O 0.3758(3) 0.2143(4) 0.0964(2) 0.0258(14) Uani 1 1 d . . .
O7 O 0.4379(3) 0.2558(4) 0.2033(2) 0.0200(12) Uani 1 1 d . . .
O8 O 0.3101(3) 0.0732(4) 0.2330(3) 0.0346(16) Uani 1 1 d . . .
O9 O 0.3059(3) 0.2156(4) 0.1639(2) 0.0235(13) Uani 1 1 d . . .
O10 O 0.2614(3) 0.3328(5) 0.0700(3) 0.0356(16) Uani 1 1 d . . .
O11 O 0.4016(3) 0.3998(4) 0.1164(2) 0.0221(13) Uani 1 1 d . . .
O12 O 0.3624(3) 0.2410(4) 0.2791(2) 0.0239(13) Uani 1 1 d . . .
O13 O 0.4638(3) 0.3847(4) 0.2845(2) 0.0171(12) Uani 1 1 d . . .
O14 O 0.3316(3) 0.3998(4) 0.1826(2) 0.0232(13) Uani 1 1 d . . .
O15 O 0.3473(3) 0.4264(4) 0.2929(2) 0.0233(13) Uani 1 1 d . . .
O16 O 0.4678(3) 0.4267(4) 0.3838(2) 0.0223(13) Uani 1 1 d . . .
O17 O 0.3621(4) 0.3059(5) 0.3821(3) 0.0369(17) Uani 1 1 d . . .
O18 O 0.5593(3) 0.5715(4) 0.4082(3) 0.0283(14) Uani 1 1 d . . .
O19 O 0.4499(3) 0.5551(4) 0.2981(2) 0.0217(13) Uani 1 1 d . . .
O20 O 0.5722(3) 0.5276(4) 0.3048(2) 0.0223(13) Uani 1 1 d . . .
O21 O 0.3069(3) 0.5694(4) 0.2184(3) 0.0291(14) Uani 1 1 d . . .
O22 O 0.5000 0.7070(7) 0.2500 0.047(3) Uani 1 2 d S . .


_geom_special_details            
; 
 All esds (except the esd in the dihedral angle between two l.s. planes) 
 are estimated using the full covariance matrix.  The cell esds are taken 
 into account individually in the estimation of esds in distances, angles 
 and torsion angles; correlations between esds in cell parameters are only 
 used when they are defined by crystal symmetry.  An approximate (isotropic) 
 treatment of cell esds is used for estimating esds involving l.s. planes. 
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
As1 O13 1.660(5) . ?
As1 O13 1.660(5) 2_655 ?
As1 O7 1.664(6) 2_655 ?
As1 O7 1.664(6) . ?
C1 N2 1.315(14) . ?
C1 N1 1.347(14) . ?
C1 H1 0.9300 . ?
C2 C3 1.323(18) . ?
C2 N1 1.390(16) . ?
C2 H2 0.9300 . ?
C3 N2 1.361(15) . ?
C3 H3 0.9300 . ?
C4 N3 1.302(15) . ?
C4 N4 1.331(15) . ?
C4 H4 0.9300 . ?
C5 C6 1.345(17) . ?
C5 N3 1.358(15) . ?
C5 H5 0.9300 . ?
C6 N4 1.338(18) . ?
C6 H6 0.9300 . ?
C7 N6 1.29(2) . ?
C7 C8 1.30(2) . ?
C7 H7 0.9300 . ?
N5 C8 1.28(2) . ?
N5 C9 1.33(2) . ?
C9 N6 1.26(2) . ?
C9 H9 0.9300 . ?
C10 N7 1.341(16) . ?
C10 C12 1.40(2) . ?
C10 H10 0.9300 . ?
C11 N7 1.297(17) . ?
C11 N8 1.32(2) . ?
C11 H11 0.9300 . ?
N8 C12 1.29(2) . ?
C13 N10 1.279(19) . ?
C13 N9 1.341(18) . ?
C13 H13 0.9300 . ?
N9 C14 1.270(19) . ?
C15 C14 1.31(2) . ?
C15 N10 1.340(19) . ?
C15 H15 0.9300 . ?
V1 O1 1.596(11) . ?
V1 O3 1.909(6) 2_655 ?
V1 O3 1.909(6) . ?
V1 O2 1.998(6) 2_655 ?
V1 O2 1.998(6) . ?
V1 Mo2 3.1002(13) . ?
V1 Mo2 3.1003(13) 2_655 ?
V1 Mo1 3.1083(13) 2_655 ?
V1 Mo1 3.1084(13) . ?
V2 O22 1.598(11) . ?
V2 O20 1.899(6) 2_655 ?
V2 O20 1.899(6) . ?
V2 O19 2.002(6) 2_655 ?
V2 O19 2.002(6) . ?
V2 Mo6 3.1042(13) 2_655 ?
V2 Mo4 3.1073(13) . ?
V2 Mo4 3.1074(13) 2_655 ?
Cu1 N2 1.878(9) . ?
Cu1 N3 1.881(9) . ?
Cu2 N6 1.882(11) . ?
Cu2 N7 1.906(10) . ?
Cu3 N10 1.864(11) . ?
Cu3 N10 1.864(11) 5_565 ?
Mo1 O4 1.684(6) . ?
Mo1 O5 1.826(6) . ?
Mo1 O6 1.837(6) . ?
Mo1 O2 2.041(6) . ?
Mo1 O3 2.059(6) . ?
Mo1 O7 2.400(6) . ?
Mo2 O8 1.673(6) . ?
Mo2 O12 1.816(6) . ?
Mo2 O9 1.860(6) . ?
Mo2 O2 2.052(6) . ?
Mo2 O3 2.053(6) 2_655 ?
Mo2 O7 2.392(5) . ?
Mo3 O10 1.648(7) . ?
Mo3 O11 1.950(6) . ?
Mo3 O14 1.953(6) . ?
Mo3 O9 1.966(6) . ?
Mo3 O6 1.974(6) . ?
Mo3 O7 2.426(6) . ?
Mo4 O21 1.677(6) . ?
Mo4 O14 1.831(6) . ?
Mo4 O15 1.836(6) . ?
Mo4 O19 2.055(6) . ?
Mo4 O20 2.060(6) 2_655 ?
Mo4 O13 2.395(5) . ?
Mo5 O17 1.645(6) . ?
Mo5 O5 1.945(6) 2_655 ?
Mo5 O12 1.955(6) . ?
Mo5 O16 1.968(6) . ?
Mo5 O15 1.976(6) . ?
Mo5 O13 2.396(5) . ?
Mo6 O18 1.684(6) . ?
Mo6 O11 1.832(6) 2_655 ?
Mo6 O16 1.840(6) . ?
Mo6 O20 2.040(6) . ?
Mo6 O19 2.042(6) . ?
Mo6 O13 2.401(5) . ?
C8 H8 0.9300 . ?
C12 H12 0.9300 . ?
C14 H14 0.9300 . ?
O3 Mo2 2.053(6) 2_655 ?
O5 Mo5 1.945(6) 2_655 ?
O11 Mo6 1.832(6) 2_655 ?
O20 Mo4 2.060(6) 2_655 ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O13 As1 O13 110.9(4) . 2_655 ?
O13 As1 O7 108.8(3) . 2_655 ?
O13 As1 O7 108.8(3) 2_655 2_655 ?
O13 As1 O7 108.8(3) . . ?
O13 As1 O7 108.8(3) 2_655 . ?
O7 As1 O7 110.8(4) 2_655 . ?
N2 C1 N1 110.8(10) . . ?
N2 C1 H1 124.6 . . ?
N1 C1 H1 124.6 . . ?
C3 C2 N1 105.9(11) . . ?
C3 C2 H2 127.1 . . ?
N1 C2 H2 127.1 . . ?
C2 C3 N2 110.9(11) . . ?
C2 C3 H3 124.5 . . ?
N2 C3 H3 124.5 . . ?
N3 C4 N4 112.7(12) . . ?
N3 C4 H4 123.6 . . ?
N4 C4 H4 123.6 . . ?
C6 C5 N3 108.4(12) . . ?
C6 C5 H5 125.8 . . ?
N3 C5 H5 125.8 . . ?
N4 C6 C5 108.2(12) . . ?
N4 C6 H6 125.9 . . ?
C5 C6 H6 125.9 . . ?
N6 C7 C8 113(2) . . ?
N6 C7 H7 123.3 . . ?
C8 C7 H7 123.3 . . ?
C8 N5 C9 104.6(16) . . ?
N6 C9 N5 113.5(19) . . ?
N6 C9 H9 123.3 . . ?
N5 C9 H9 123.3 . . ?
N7 C10 C12 105.6(14) . . ?
N7 C10 H10 127.2 . . ?
C12 C10 H10 127.2 . . ?
N7 C11 N8 109.7(16) . . ?
N7 C11 H11 125.2 . . ?
N8 C11 H11 125.2 . . ?
C12 N8 C11 109.3(15) . . ?
N10 C13 N9 111.7(14) . . ?
N10 C13 H13 124.2 . . ?
N9 C13 H13 124.2 . . ?
C14 N9 C13 106.7(13) . . ?
C14 C15 N10 110.5(14) . . ?
C14 C15 H15 124.7 . . ?
N10 C15 H15 124.7 . . ?
O1 V1 O3 121.58(19) . 2_655 ?
O1 V1 O3 121.58(18) . . ?
O3 V1 O3 116.8(4) 2_655 . ?
O1 V1 O2 108.21(18) . 2_655 ?
O3 V1 O2 80.3(2) 2_655 2_655 ?
O3 V1 O2 80.9(2) . 2_655 ?
O1 V1 O2 108.21(18) . . ?
O3 V1 O2 80.9(2) 2_655 . ?
O3 V1 O2 80.3(2) . . ?
O2 V1 O2 143.6(4) 2_655 . ?
O1 V1 Mo2 121.66(4) . . ?
O3 V1 Mo2 40.21(18) 2_655 . ?
O3 V1 Mo2 102.36(19) . . ?
O2 V1 Mo2 115.47(18) 2_655 . ?
O2 V1 Mo2 40.71(17) . . ?
O1 V1 Mo2 121.66(4) . 2_655 ?
O3 V1 Mo2 102.36(19) 2_655 2_655 ?
O3 V1 Mo2 40.21(18) . 2_655 ?
O2 V1 Mo2 40.71(17) 2_655 2_655 ?
O2 V1 Mo2 115.47(18) . 2_655 ?
Mo2 V1 Mo2 116.69(7) . 2_655 ?
O1 V1 Mo1 121.32(4) . 2_655 ?
O3 V1 Mo1 40.19(18) 2_655 2_655 ?
O3 V1 Mo1 102.68(19) . 2_655 ?
O2 V1 Mo1 40.20(17) 2_655 2_655 ?
O2 V1 Mo1 116.04(18) . 2_655 ?
Mo2 V1 Mo1 77.99(4) . 2_655 ?
Mo2 V1 Mo1 70.27(3) 2_655 2_655 ?
O1 V1 Mo1 121.32(4) . . ?
O3 V1 Mo1 102.68(19) 2_655 . ?
O3 V1 Mo1 40.19(18) . . ?
O2 V1 Mo1 116.04(18) 2_655 . ?
O2 V1 Mo1 40.20(17) . . ?
Mo2 V1 Mo1 70.27(3) . . ?
Mo2 V1 Mo1 77.99(4) 2_655 . ?
Mo1 V1 Mo1 117.35(7) 2_655 . ?
O22 V2 O20 122.78(18) . 2_655 ?
O22 V2 O20 122.78(18) . . ?
O20 V2 O20 114.4(4) 2_655 . ?
O22 V2 O19 108.21(17) . 2_655 ?
O20 V2 O19 79.8(2) 2_655 2_655 ?
O20 V2 O19 80.7(2) . 2_655 ?
O22 V2 O19 108.21(17) . . ?
O20 V2 O19 80.7(2) 2_655 . ?
O20 V2 O19 79.8(2) . . ?
O19 V2 O19 143.6(3) 2_655 . ?
O22 V2 Mo6 121.54(3) . 2_655 ?
O20 V2 Mo6 39.62(17) 2_655 2_655 ?
O20 V2 Mo6 101.76(18) . 2_655 ?
O19 V2 Mo6 40.34(16) 2_655 2_655 ?
O19 V2 Mo6 115.80(17) . 2_655 ?
O22 V2 Mo4 121.72(3) . . ?
O20 V2 Mo4 40.17(17) 2_655 . ?
O20 V2 Mo4 101.23(18) . . ?
O19 V2 Mo4 115.48(18) 2_655 . ?
O19 V2 Mo4 40.63(16) . . ?
Mo6 V2 Mo4 77.83(4) 2_655 . ?
O22 V2 Mo4 121.72(3) . 2_655 ?
O20 V2 Mo4 101.23(18) 2_655 2_655 ?
O20 V2 Mo4 40.17(17) . 2_655 ?
O19 V2 Mo4 40.63(16) 2_655 2_655 ?
O19 V2 Mo4 115.48(18) . 2_655 ?
Mo6 V2 Mo4 70.17(3) 2_655 2_655 ?
Mo4 V2 Mo4 116.55(7) . 2_655 ?
N2 Cu1 N3 175.8(5) . . ?
N6 Cu2 N7 167.4(6) . . ?
N10 Cu3 N10 179.997(1) . 5_565 ?
O4 Mo1 O5 104.8(3) . . ?
O4 Mo1 O6 101.8(3) . . ?
O5 Mo1 O6 96.6(3) . . ?
O4 Mo1 O2 100.7(3) . . ?
O5 Mo1 O2 150.4(3) . . ?
O6 Mo1 O2 92.8(3) . . ?
O4 Mo1 O3 99.0(3) . . ?
O5 Mo1 O3 85.3(3) . . ?
O6 Mo1 O3 157.9(2) . . ?
O2 Mo1 O3 75.8(2) . . ?
O4 Mo1 O7 168.6(3) . . ?
O5 Mo1 O7 86.4(2) . . ?
O6 Mo1 O7 74.3(2) . . ?
O2 Mo1 O7 69.2(2) . . ?
O3 Mo1 O7 83.8(2) . . ?
O4 Mo1 V1 100.8(2) . . ?
O5 Mo1 V1 119.63(19) . . ?
O6 Mo1 V1 130.01(19) . . ?
O2 Mo1 V1 39.18(17) . . ?
O3 Mo1 V1 36.74(16) . . ?
O7 Mo1 V1 74.88(14) . . ?
O8 Mo2 O12 104.2(3) . . ?
O8 Mo2 O9 100.3(3) . . ?
O12 Mo2 O9 96.4(3) . . ?
O8 Mo2 O2 100.4(3) . . ?
O12 Mo2 O2 152.1(2) . . ?
O9 Mo2 O2 91.9(3) . . ?
O8 Mo2 O3 100.4(3) . 2_655 ?
O12 Mo2 O3 86.5(3) . 2_655 ?
O9 Mo2 O3 157.7(2) . 2_655 ?
O2 Mo2 O3 76.2(2) . 2_655 ?
O8 Mo2 O7 167.3(3) . . ?
O12 Mo2 O7 87.7(2) . . ?
O9 Mo2 O7 73.6(2) . . ?
O2 Mo2 O7 69.2(2) . . ?
O3 Mo2 O7 84.4(2) 2_655 . ?
O8 Mo2 V1 101.7(2) . . ?
O12 Mo2 V1 121.07(19) . . ?
O9 Mo2 V1 129.33(18) . . ?
O2 Mo2 V1 39.41(17) . . ?
O3 Mo2 V1 36.87(16) 2_655 . ?
O7 Mo2 V1 75.15(14) . . ?
O10 Mo3 O11 104.2(3) . . ?
O10 Mo3 O14 104.1(3) . . ?
O11 Mo3 O14 84.9(2) . . ?
O10 Mo3 O9 101.2(3) . . ?
O11 Mo3 O9 154.7(2) . . ?
O14 Mo3 O9 89.3(2) . . ?
O10 Mo3 O6 100.7(3) . . ?
O11 Mo3 O6 90.1(2) . . ?
O14 Mo3 O6 155.1(3) . . ?
O9 Mo3 O6 84.9(3) . . ?
O10 Mo3 O7 169.2(3) . . ?
O11 Mo3 O7 83.7(2) . . ?
O14 Mo3 O7 83.7(2) . . ?
O9 Mo3 O7 71.1(2) . . ?
O6 Mo3 O7 71.6(2) . . ?
O21 Mo4 O14 103.9(3) . . ?
O21 Mo4 O15 102.1(3) . . ?
O14 Mo4 O15 96.9(3) . . ?
O21 Mo4 O19 99.9(3) . . ?
O14 Mo4 O19 152.0(2) . . ?
O15 Mo4 O19 92.1(2) . . ?
O21 Mo4 O20 99.5(3) . 2_655 ?
O14 Mo4 O20 86.0(2) . 2_655 ?
O15 Mo4 O20 156.8(2) . 2_655 ?
O19 Mo4 O20 75.8(2) . 2_655 ?
O21 Mo4 O13 168.2(3) . . ?
O14 Mo4 O13 87.7(2) . . ?
O15 Mo4 O13 73.9(2) . . ?
O19 Mo4 O13 69.5(2) . . ?
O20 Mo4 O13 83.3(2) 2_655 . ?
O21 Mo4 V2 100.1(2) . . ?
O14 Mo4 V2 120.66(17) . . ?
O15 Mo4 V2 129.48(19) . . ?
O19 Mo4 V2 39.39(16) . . ?
O20 Mo4 V2 36.49(16) 2_655 . ?
O13 Mo4 V2 75.25(14) . . ?
O17 Mo5 O5 103.2(3) . 2_655 ?
O17 Mo5 O12 102.3(3) . . ?
O5 Mo5 O12 85.1(3) 2_655 . ?
O17 Mo5 O16 101.3(3) . . ?
O5 Mo5 O16 90.5(3) 2_655 . ?
O12 Mo5 O16 156.3(2) . . ?
O17 Mo5 O15 101.3(3) . . ?
O5 Mo5 O15 155.5(2) 2_655 . ?
O12 Mo5 O15 89.6(3) . . ?
O16 Mo5 O15 84.9(2) . . ?
O17 Mo5 O13 170.5(3) . . ?
O5 Mo5 O13 84.0(2) 2_655 . ?
O12 Mo5 O13 84.3(2) . . ?
O16 Mo5 O13 72.2(2) . . ?
O15 Mo5 O13 71.7(2) . . ?
O18 Mo6 O11 104.9(3) . 2_655 ?
O18 Mo6 O16 102.3(3) . . ?
O11 Mo6 O16 96.4(3) 2_655 . ?
O18 Mo6 O20 99.2(3) . . ?
O11 Mo6 O20 86.1(2) 2_655 . ?
O16 Mo6 O20 156.9(2) . . ?
O18 Mo6 O19 99.3(3) . . ?
O11 Mo6 O19 151.7(2) 2_655 . ?
O16 Mo6 O19 92.4(2) . . ?
O20 Mo6 O19 75.7(2) . . ?
O18 Mo6 O13 167.8(3) . . ?
O11 Mo6 O13 87.2(2) 2_655 . ?
O16 Mo6 O13 74.0(2) . . ?
O20 Mo6 O13 83.2(2) . . ?
O19 Mo6 O13 69.5(2) . . ?
C1 N1 C2 106.6(10) . . ?
C1 N2 C3 105.9(10) . . ?
C1 N2 Cu1 127.3(8) . . ?
C3 N2 Cu1 126.8(8) . . ?
C4 N3 C5 105.2(10) . . ?
C4 N3 Cu1 126.4(9) . . ?
C5 N3 Cu1 128.3(8) . . ?
C4 N4 C6 105.5(10) . . ?
N5 C8 C7 106.0(19) . . ?
N5 C8 H8 127.0 . . ?
C7 C8 H8 127.0 . . ?
C9 N6 C7 102.0(15) . . ?
C9 N6 Cu2 127.8(13) . . ?
C7 N6 Cu2 129.8(13) . . ?
C11 N7 C10 108.3(13) . . ?
C11 N7 Cu2 124.4(10) . . ?
C10 N7 Cu2 127.0(9) . . ?
N8 C12 C10 107.0(13) . . ?
N8 C12 H12 126.5 . . ?
C10 C12 H12 126.5 . . ?
N9 C14 C15 107.7(14) . . ?
N9 C14 H14 126.2 . . ?
C15 C14 H14 126.2 . . ?
C13 N10 C15 103.3(13) . . ?
C13 N10 Cu3 127.9(12) . . ?
C15 N10 Cu3 128.2(11) . . ?
V1 O2 Mo1 100.6(3) . . ?
V1 O2 Mo2 99.9(3) . . ?
Mo1 O2 Mo2 121.6(3) . . ?
V1 O3 Mo2 102.9(3) . 2_655 ?
V1 O3 Mo1 103.1(3) . . ?
Mo2 O3 Mo1 143.6(3) 2_655 . ?
Mo1 O5 Mo5 156.1(3) . 2_655 ?
Mo1 O6 Mo3 125.0(3) . . ?
As1 O7 Mo2 123.2(3) . . ?
As1 O7 Mo1 123.9(3) . . ?
Mo2 O7 Mo1 96.4(2) . . ?
As1 O7 Mo3 124.9(3) . . ?
Mo2 O7 Mo3 89.75(19) . . ?
Mo1 O7 Mo3 88.94(19) . . ?
Mo2 O9 Mo3 125.4(3) . . ?
Mo6 O11 Mo3 155.3(3) 2_655 . ?
Mo2 O12 Mo5 154.2(3) . . ?
As1 O13 Mo4 123.5(3) . . ?
As1 O13 Mo5 125.0(3) . . ?
Mo4 O13 Mo5 89.61(18) . . ?
As1 O13 Mo6 123.7(3) . . ?
Mo4 O13 Mo6 96.2(2) . . ?
Mo5 O13 Mo6 89.20(17) . . ?
Mo4 O14 Mo3 155.0(3) . . ?
Mo4 O15 Mo5 124.6(3) . . ?
Mo6 O16 Mo5 124.4(3) . . ?
V2 O19 Mo6 100.3(3) . . ?
V2 O19 Mo4 100.0(2) . . ?
Mo6 O19 Mo4 121.3(3) . . ?
V2 O20 Mo6 104.0(3) . . ?
V2 O20 Mo4 103.3(3) . 2_655 ?
Mo6 O20 Mo4 144.2(3) . 2_655 ?

loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion_publ_flag
N1 C2 C3 N2 -1(2) . . . . ?
N3 C5 C6 N4 -1.1(16) . . . . ?
C8 N5 C9 N6 3(3) . . . . ?
N7 C11 N8 C12 1(2) . . . . ?
N10 C13 N9 C14 1(3) . . . . ?
O1 V1 Mo1 O4 -12.6(2) . . . . ?
O3 V1 Mo1 O4 -152.5(3) 2_655 . . . ?
O3 V1 Mo1 O4 90.7(4) . . . . ?
O2 V1 Mo1 O4 122.2(3) 2_655 . . . ?
O2 V1 Mo1 O4 -93.7(4) . . . . ?
Mo2 V1 Mo1 O4 -128.3(2) . . . . ?
Mo2 V1 Mo1 O4 107.3(2) 2_655 . . . ?
Mo1 V1 Mo1 O4 167.4(2) 2_655 . . . ?
O1 V1 Mo1 O5 -126.6(2) . . . . ?
O3 V1 Mo1 O5 93.5(3) 2_655 . . . ?
O3 V1 Mo1 O5 -23.3(4) . . . . ?
O2 V1 Mo1 O5 8.2(3) 2_655 . . . ?
O2 V1 Mo1 O5 152.2(3) . . . . ?
Mo2 V1 Mo1 O5 117.7(2) . . . . ?
Mo2 V1 Mo1 O5 -6.7(2) 2_655 . . . ?
Mo1 V1 Mo1 O5 53.4(2) 2_655 . . . ?
O1 V1 Mo1 O6 103.0(2) . . . . ?
O3 V1 Mo1 O6 -37.0(3) 2_655 . . . ?
O3 V1 Mo1 O6 -153.8(4) . . . . ?
O2 V1 Mo1 O6 -122.3(3) 2_655 . . . ?
O2 V1 Mo1 O6 21.8(4) . . . . ?
Mo2 V1 Mo1 O6 -12.8(2) . . . . ?
Mo2 V1 Mo1 O6 -137.1(2) 2_655 . . . ?
Mo1 V1 Mo1 O6 -77.0(2) 2_655 . . . ?
O1 V1 Mo1 O2 81.2(3) . . . . ?
O3 V1 Mo1 O2 -58.8(3) 2_655 . . . ?
O3 V1 Mo1 O2 -175.6(4) . . . . ?
O2 V1 Mo1 O2 -144.1(4) 2_655 . . . ?
Mo2 V1 Mo1 O2 -34.6(3) . . . . ?
Mo2 V1 Mo1 O2 -158.9(3) 2_655 . . . ?
Mo1 V1 Mo1 O2 -98.8(3) 2_655 . . . ?
O1 V1 Mo1 O3 -103.3(3) . . . . ?
O3 V1 Mo1 O3 116.8(4) 2_655 . . . ?
O2 V1 Mo1 O3 31.5(3) 2_655 . . . ?
O2 V1 Mo1 O3 175.6(4) . . . . ?
Mo2 V1 Mo1 O3 141.0(3) . . . . ?
Mo2 V1 Mo1 O3 16.6(3) 2_655 . . . ?
Mo1 V1 Mo1 O3 76.7(3) 2_655 . . . ?
O1 V1 Mo1 O7 156.62(13) . . . . ?
O3 V1 Mo1 O7 16.7(2) 2_655 . . . ?
O3 V1 Mo1 O7 -100.1(3) . . . . ?
O2 V1 Mo1 O7 -68.6(2) 2_655 . . . ?
O2 V1 Mo1 O7 75.5(3) . . . . ?
Mo2 V1 Mo1 O7 40.88(14) . . . . ?
Mo2 V1 Mo1 O7 -83.46(14) 2_655 . . . ?
Mo1 V1 Mo1 O7 -23.37(13) 2_655 . . . ?
O1 V1 Mo2 O8 11.0(2) . . . . ?
O3 V1 Mo2 O8 -91.9(4) 2_655 . . . ?
O3 V1 Mo2 O8 150.9(3) . . . . ?
O2 V1 Mo2 O8 -123.4(3) 2_655 . . . ?
O2 V1 Mo2 O8 92.2(4) . . . . ?
Mo2 V1 Mo2 O8 -169.0(2) 2_655 . . . ?
Mo1 V1 Mo2 O8 -108.5(2) 2_655 . . . ?
Mo1 V1 Mo2 O8 126.4(2) . . . . ?
O1 V1 Mo2 O12 125.7(2) . . . . ?
O3 V1 Mo2 O12 22.7(4) 2_655 . . . ?
O3 V1 Mo2 O12 -94.4(3) . . . . ?
O2 V1 Mo2 O12 -8.8(3) 2_655 . . . ?
O2 V1 Mo2 O12 -153.2(3) . . . . ?
Mo2 V1 Mo2 O12 -54.3(2) 2_655 . . . ?
Mo1 V1 Mo2 O12 6.1(2) 2_655 . . . ?
Mo1 V1 Mo2 O12 -119.0(2) . . . . ?
O1 V1 Mo2 O9 -102.9(2) . . . . ?
O3 V1 Mo2 O9 154.2(4) 2_655 . . . ?
O3 V1 Mo2 O9 37.0(3) . . . . ?
O2 V1 Mo2 O9 122.7(3) 2_655 . . . ?
O2 V1 Mo2 O9 -21.7(4) . . . . ?
Mo2 V1 Mo2 O9 77.1(2) 2_655 . . . ?
Mo1 V1 Mo2 O9 137.6(2) 2_655 . . . ?
Mo1 V1 Mo2 O9 12.4(2) . . . . ?
O1 V1 Mo2 O2 -81.1(3) . . . . ?
O3 V1 Mo2 O2 175.9(4) 2_655 . . . ?
O3 V1 Mo2 O2 58.7(3) . . . . ?
O2 V1 Mo2 O2 144.4(4) 2_655 . . . ?
Mo2 V1 Mo2 O2 98.8(3) 2_655 . . . ?
Mo1 V1 Mo2 O2 159.3(3) 2_655 . . . ?
Mo1 V1 Mo2 O2 34.2(3) . . . . ?
O1 V1 Mo2 O3 102.9(3) . . . 2_655 ?
O3 V1 Mo2 O3 -117.2(4) . . . 2_655 ?
O2 V1 Mo2 O3 -31.5(3) 2_655 . . 2_655 ?
O2 V1 Mo2 O3 -175.9(4) . . . 2_655 ?
Mo2 V1 Mo2 O3 -77.1(3) 2_655 . . 2_655 ?
Mo1 V1 Mo2 O3 -16.6(3) 2_655 . . 2_655 ?
Mo1 V1 Mo2 O3 -141.8(3) . . . 2_655 ?
O1 V1 Mo2 O7 -156.32(14) . . . . ?
O3 V1 Mo2 O7 100.8(3) 2_655 . . . ?
O3 V1 Mo2 O7 -16.4(2) . . . . ?
O2 V1 Mo2 O7 69.2(2) 2_655 . . . ?
O2 V1 Mo2 O7 -75.2(3) . . . . ?
Mo2 V1 Mo2 O7 23.68(14) 2_655 . . . ?
Mo1 V1 Mo2 O7 84.13(14) 2_655 . . . ?
Mo1 V1 Mo2 O7 -41.00(14) . . . . ?
O22 V2 Mo4 O21 12.4(2) . . . . ?
O20 V2 Mo4 O21 -92.3(3) 2_655 . . . ?
O20 V2 Mo4 O21 152.9(3) . . . . ?
O19 V2 Mo4 O21 -122.2(3) 2_655 . . . ?
O19 V2 Mo4 O21 93.4(3) . . . . ?
Mo6 V2 Mo4 O21 -107.3(2) 2_655 . . . ?
Mo4 V2 Mo4 O21 -167.6(2) 2_655 . . . ?
O22 V2 Mo4 O14 125.3(2) . . . . ?
O20 V2 Mo4 O14 20.6(4) 2_655 . . . ?
O20 V2 Mo4 O14 -94.2(3) . . . . ?
O19 V2 Mo4 O14 -9.2(3) 2_655 . . . ?
O19 V2 Mo4 O14 -153.7(3) . . . . ?
Mo6 V2 Mo4 O14 5.6(2) 2_655 . . . ?
Mo4 V2 Mo4 O14 -54.7(2) 2_655 . . . ?
O22 V2 Mo4 O15 -102.6(2) . . . . ?
O20 V2 Mo4 O15 152.7(4) 2_655 . . . ?
O20 V2 Mo4 O15 37.9(3) . . . . ?
O19 V2 Mo4 O15 122.9(3) 2_655 . . . ?
O19 V2 Mo4 O15 -21.6(3) . . . . ?
Mo6 V2 Mo4 O15 137.7(2) 2_655 . . . ?
Mo4 V2 Mo4 O15 77.4(2) 2_655 . . . ?
O22 V2 Mo4 O19 -81.0(3) . . . . ?
O20 V2 Mo4 O19 174.2(4) 2_655 . . . ?
O20 V2 Mo4 O19 59.5(3) . . . . ?
O19 V2 Mo4 O19 144.4(3) 2_655 . . . ?
Mo6 V2 Mo4 O19 159.3(3) 2_655 . . . ?
Mo4 V2 Mo4 O19 99.0(3) 2_655 . . . ?
O22 V2 Mo4 O20 104.7(3) . . . 2_655 ?
O20 V2 Mo4 O20 -114.7(4) . . . 2_655 ?
O19 V2 Mo4 O20 -29.8(3) 2_655 . . 2_655 ?
O19 V2 Mo4 O20 -174.2(4) . . . 2_655 ?
Mo6 V2 Mo4 O20 -15.0(3) 2_655 . . 2_655 ?
Mo4 V2 Mo4 O20 -75.3(3) 2_655 . . 2_655 ?
O22 V2 Mo4 O13 -156.50(13) . . . . ?
O20 V2 Mo4 O13 98.8(3) 2_655 . . . ?
O20 V2 Mo4 O13 -16.0(2) . . . . ?
O19 V2 Mo4 O13 68.9(2) 2_655 . . . ?
O19 V2 Mo4 O13 -75.5(3) . . . . ?
Mo6 V2 Mo4 O13 83.78(13) 2_655 . . . ?
Mo4 V2 Mo4 O13 23.50(13) 2_655 . . . ?
N2 C1 N1 C2 -0.1(16) . . . . ?
C3 C2 N1 C1 0.8(19) . . . . ?
N1 C1 N2 C3 -0.6(16) . . . . ?
N1 C1 N2 Cu1 -179.8(9) . . . . ?
C2 C3 N2 C1 1(2) . . . . ?
C2 C3 N2 Cu1 -179.7(12) . . . . ?
N3 Cu1 N2 C1 123(5) . . . . ?
N3 Cu1 N2 C3 -56(6) . . . . ?
N4 C4 N3 C5 -1.6(16) . . . . ?
N4 C4 N3 Cu1 -177.8(9) . . . . ?
C6 C5 N3 C4 1.7(15) . . . . ?
C6 C5 N3 Cu1 177.7(9) . . . . ?
N2 Cu1 N3 C4 -119(6) . . . . ?
N2 Cu1 N3 C5 65(6) . . . . ?
N3 C4 N4 C6 0.9(16) . . . . ?
C5 C6 N4 C4 0.2(16) . . . . ?
C9 N5 C8 C7 1(3) . . . . ?
N6 C7 C8 N5 -5(4) . . . . ?
N5 C9 N6 C7 -6(3) . . . . ?
N5 C9 N6 Cu2 -178.9(14) . . . . ?
C8 C7 N6 C9 7(3) . . . . ?
C8 C7 N6 Cu2 179.7(19) . . . . ?
N7 Cu2 N6 C9 -123(3) . . . . ?
N7 Cu2 N6 C7 66(4) . . . . ?
N8 C11 N7 C10 0.6(19) . . . . ?
N8 C11 N7 Cu2 174.3(12) . . . . ?
C12 C10 N7 C11 -1.8(17) . . . . ?
C12 C10 N7 Cu2 -175.2(10) . . . . ?
N6 Cu2 N7 C11 86(3) . . . . ?
N6 Cu2 N7 C10 -102(3) . . . . ?
C11 N8 C12 C10 -2(2) . . . . ?
N7 C10 C12 N8 2(2) . . . . ?
C13 N9 C14 C15 2(2) . . . . ?
N10 C15 C14 N9 -3(2) . . . . ?
N9 C13 N10 C15 -2(2) . . . . ?
N9 C13 N10 Cu3 169.2(13) . . . . ?
C14 C15 N10 C13 3(2) . . . . ?
C14 C15 N10 Cu3 -168.1(14) . . . . ?
N10 Cu3 N10 C13 26(4) 5_565 . . . ?
N10 Cu3 N10 C15 -164(4) 5_565 . . . ?
O1 V1 O2 Mo1 -117.30(19) . . . . ?
O3 V1 O2 Mo1 122.3(3) 2_655 . . . ?
O3 V1 O2 Mo1 2.9(3) . . . . ?
O2 V1 O2 Mo1 62.70(18) 2_655 . . . ?
Mo2 V1 O2 Mo1 125.0(4) . . . . ?
Mo2 V1 O2 Mo1 22.9(3) 2_655 . . . ?
Mo1 V1 O2 Mo1 102.4(2) 2_655 . . . ?
O1 V1 O2 Mo2 117.70(18) . . . . ?
O3 V1 O2 Mo2 -2.7(2) 2_655 . . . ?
O3 V1 O2 Mo2 -122.1(3) . . . . ?
O2 V1 O2 Mo2 -62.30(18) 2_655 . . . ?
Mo2 V1 O2 Mo2 -102.1(2) 2_655 . . . ?
Mo1 V1 O2 Mo2 -22.6(3) 2_655 . . . ?
Mo1 V1 O2 Mo2 -125.0(4) . . . . ?
O4 Mo1 O2 V1 94.0(3) . . . . ?
O5 Mo1 O2 V1 -54.9(6) . . . . ?
O6 Mo1 O2 V1 -163.5(3) . . . . ?
O3 Mo1 O2 V1 -2.7(2) . . . . ?
O7 Mo1 O2 V1 -91.4(3) . . . . ?
O4 Mo1 O2 Mo2 -157.3(4) . . . . ?
O5 Mo1 O2 Mo2 53.7(7) . . . . ?
O6 Mo1 O2 Mo2 -54.8(4) . . . . ?
O3 Mo1 O2 Mo2 106.0(4) . . . . ?
O7 Mo1 O2 Mo2 17.3(3) . . . . ?
V1 Mo1 O2 Mo2 108.7(4) . . . . ?
O8 Mo2 O2 V1 -95.8(3) . . . . ?
O12 Mo2 O2 V1 55.7(6) . . . . ?
O9 Mo2 O2 V1 163.3(3) . . . . ?
O3 Mo2 O2 V1 2.5(2) 2_655 . . . ?
O7 Mo2 O2 V1 91.7(3) . . . . ?
O8 Mo2 O2 Mo1 155.1(4) . . . . ?
O12 Mo2 O2 Mo1 -53.3(7) . . . . ?
O9 Mo2 O2 Mo1 54.3(4) . . . . ?
O3 Mo2 O2 Mo1 -106.6(4) 2_655 . . . ?
O7 Mo2 O2 Mo1 -17.3(3) . . . . ?
V1 Mo2 O2 Mo1 -109.1(4) . . . . ?
O1 V1 O3 Mo2 -103.1(2) . . . 2_655 ?
O3 V1 O3 Mo2 76.9(2) 2_655 . . 2_655 ?
O2 V1 O3 Mo2 2.7(3) 2_655 . . 2_655 ?
O2 V1 O3 Mo2 151.4(3) . . . 2_655 ?
Mo2 V1 O3 Mo2 116.9(2) . . . 2_655 ?
Mo1 V1 O3 Mo2 36.7(2) 2_655 . . 2_655 ?
Mo1 V1 O3 Mo2 154.3(4) . . . 2_655 ?
O1 V1 O3 Mo1 102.6(2) . . . . ?
O3 V1 O3 Mo1 -77.4(2) 2_655 . . . ?
O2 V1 O3 Mo1 -151.6(3) 2_655 . . . ?
O2 V1 O3 Mo1 -2.9(3) . . . . ?
Mo2 V1 O3 Mo1 -37.3(2) . . . . ?
Mo2 V1 O3 Mo1 -154.3(4) 2_655 . . . ?
Mo1 V1 O3 Mo1 -117.6(2) 2_655 . . . ?
O4 Mo1 O3 V1 -95.9(3) . . . . ?
O5 Mo1 O3 V1 159.8(3) . . . . ?
O6 Mo1 O3 V1 63.9(8) . . . . ?
O2 Mo1 O3 V1 2.9(3) . . . . ?
O7 Mo1 O3 V1 72.9(3) . . . . ?
O4 Mo1 O3 Mo2 129.5(5) . . . 2_655 ?
O5 Mo1 O3 Mo2 25.2(5) . . . 2_655 ?
O6 Mo1 O3 Mo2 -70.7(9) . . . 2_655 ?
O2 Mo1 O3 Mo2 -131.7(5) . . . 2_655 ?
O7 Mo1 O3 Mo2 -61.6(5) . . . 2_655 ?
V1 Mo1 O3 Mo2 -134.6(7) . . . 2_655 ?
O4 Mo1 O5 Mo5 -129.9(9) . . . 2_655 ?
O6 Mo1 O5 Mo5 126.1(9) . . . 2_655 ?
O2 Mo1 O5 Mo5 18.5(13) . . . 2_655 ?
O3 Mo1 O5 Mo5 -31.8(9) . . . 2_655 ?
O7 Mo1 O5 Mo5 52.3(9) . . . 2_655 ?
V1 Mo1 O5 Mo5 -18.0(10) . . . 2_655 ?
O4 Mo1 O6 Mo3 173.4(4) . . . . ?
O5 Mo1 O6 Mo3 -79.9(4) . . . . ?
O2 Mo1 O6 Mo3 71.9(4) . . . . ?
O3 Mo1 O6 Mo3 13.8(9) . . . . ?
O7 Mo1 O6 Mo3 4.4(3) . . . . ?
V1 Mo1 O6 Mo3 58.3(5) . . . . ?
O10 Mo3 O6 Mo1 -176.7(4) . . . . ?
O11 Mo3 O6 Mo1 78.9(4) . . . . ?
O14 Mo3 O6 Mo1 1.0(8) . . . . ?
O9 Mo3 O6 Mo1 -76.2(4) . . . . ?
O7 Mo3 O6 Mo1 -4.5(3) . . . . ?
O13 As1 O7 Mo2 -56.1(4) . . . . ?
O13 As1 O7 Mo2 -177.0(3) 2_655 . . . ?
O7 As1 O7 Mo2 63.4(3) 2_655 . . . ?
O13 As1 O7 Mo1 176.9(3) . . . . ?
O13 As1 O7 Mo1 56.0(4) 2_655 . . . ?
O7 As1 O7 Mo1 -63.5(3) 2_655 . . . ?
O13 As1 O7 Mo3 60.7(4) . . . . ?
O13 As1 O7 Mo3 -60.2(4) 2_655 . . . ?
O7 As1 O7 Mo3 -179.8(4) 2_655 . . . ?
O8 Mo2 O7 As1 -161.5(11) . . . . ?
O12 Mo2 O7 As1 38.4(4) . . . . ?
O9 Mo2 O7 As1 135.8(4) . . . . ?
O2 Mo2 O7 As1 -125.6(4) . . . . ?
O3 Mo2 O7 As1 -48.3(4) 2_655 . . . ?
V1 Mo2 O7 As1 -84.6(3) . . . . ?
O8 Mo2 O7 Mo1 -23.4(13) . . . . ?
O12 Mo2 O7 Mo1 176.6(2) . . . . ?
O9 Mo2 O7 Mo1 -86.1(2) . . . . ?
O2 Mo2 O7 Mo1 12.5(2) . . . . ?
O3 Mo2 O7 Mo1 89.9(2) 2_655 . . . ?
V1 Mo2 O7 Mo1 53.58(14) . . . . ?
O8 Mo2 O7 Mo3 65.5(13) . . . . ?
O12 Mo2 O7 Mo3 -94.5(2) . . . . ?
O9 Mo2 O7 Mo3 2.8(2) . . . . ?
O2 Mo2 O7 Mo3 101.4(2) . . . . ?
O3 Mo2 O7 Mo3 178.8(2) 2_655 . . . ?
V1 Mo2 O7 Mo3 142.48(16) . . . . ?
O4 Mo1 O7 As1 153.2(13) . . . . ?
O5 Mo1 O7 As1 -37.7(4) . . . . ?
O6 Mo1 O7 As1 -135.6(4) . . . . ?
O2 Mo1 O7 As1 125.1(4) . . . . ?
O3 Mo1 O7 As1 48.0(4) . . . . ?
V1 Mo1 O7 As1 84.3(3) . . . . ?
O4 Mo1 O7 Mo2 15.4(15) . . . . ?
O5 Mo1 O7 Mo2 -175.5(2) . . . . ?
O6 Mo1 O7 Mo2 86.7(3) . . . . ?
O2 Mo1 O7 Mo2 -12.6(2) . . . . ?
O3 Mo1 O7 Mo2 -89.8(2) . . . . ?
V1 Mo1 O7 Mo2 -53.47(14) . . . . ?
O4 Mo1 O7 Mo3 -74.2(15) . . . . ?
O5 Mo1 O7 Mo3 94.9(2) . . . . ?
O6 Mo1 O7 Mo3 -3.0(2) . . . . ?
O2 Mo1 O7 Mo3 -102.3(2) . . . . ?
O3 Mo1 O7 Mo3 -179.4(2) . . . . ?
V1 Mo1 O7 Mo3 -143.11(16) . . . . ?
O10 Mo3 O7 As1 -180(100) . . . . ?
O11 Mo3 O7 As1 42.5(3) . . . . ?
O14 Mo3 O7 As1 -43.0(3) . . . . ?
O9 Mo3 O7 As1 -134.4(4) . . . . ?
O6 Mo3 O7 As1 134.7(4) . . . . ?
O10 Mo3 O7 Mo2 -48.1(15) . . . . ?
O11 Mo3 O7 Mo2 174.2(2) . . . . ?
O14 Mo3 O7 Mo2 88.7(2) . . . . ?
O9 Mo3 O7 Mo2 -2.7(2) . . . . ?
O6 Mo3 O7 Mo2 -93.6(2) . . . . ?
O10 Mo3 O7 Mo1 48.3(15) . . . . ?
O11 Mo3 O7 Mo1 -89.4(2) . . . . ?
O14 Mo3 O7 Mo1 -174.9(2) . . . . ?
O9 Mo3 O7 Mo1 93.7(2) . . . . ?
O6 Mo3 O7 Mo1 2.8(2) . . . . ?
O8 Mo2 O9 Mo3 -172.9(4) . . . . ?
O12 Mo2 O9 Mo3 81.4(4) . . . . ?
O2 Mo2 O9 Mo3 -72.0(4) . . . . ?
O3 Mo2 O9 Mo3 -15.0(9) 2_655 . . . ?
O7 Mo2 O9 Mo3 -4.3(3) . . . . ?
V1 Mo2 O9 Mo3 -58.3(4) . . . . ?
O10 Mo3 O9 Mo2 176.5(4) . . . . ?
O11 Mo3 O9 Mo2 -2.8(8) . . . . ?
O14 Mo3 O9 Mo2 -79.2(4) . . . . ?
O6 Mo3 O9 Mo2 76.5(4) . . . . ?
O7 Mo3 O9 Mo2 4.3(3) . . . . ?
O10 Mo3 O11 Mo6 133.8(8) . . . 2_655 ?
O14 Mo3 O11 Mo6 30.5(8) . . . 2_655 ?
O9 Mo3 O11 Mo6 -46.8(12) . . . 2_655 ?
O6 Mo3 O11 Mo6 -125.1(9) . . . 2_655 ?
O7 Mo3 O11 Mo6 -53.6(8) . . . 2_655 ?
O8 Mo2 O12 Mo5 132.6(8) . . . . ?
O9 Mo2 O12 Mo5 -125.0(8) . . . . ?
O2 Mo2 O12 Mo5 -18.5(12) . . . . ?
O3 Mo2 O12 Mo5 32.8(8) 2_655 . . . ?
O7 Mo2 O12 Mo5 -51.8(8) . . . . ?
V1 Mo2 O12 Mo5 19.3(9) . . . . ?
O17 Mo5 O12 Mo2 -133.7(8) . . . . ?
O5 Mo5 O12 Mo2 -31.3(8) 2_655 . . . ?
O16 Mo5 O12 Mo2 48.6(12) . . . . ?
O15 Mo5 O12 Mo2 124.7(8) . . . . ?
O13 Mo5 O12 Mo2 53.1(8) . . . . ?
O13 As1 O13 Mo4 63.4(3) 2_655 . . . ?
O7 As1 O13 Mo4 -177.0(3) 2_655 . . . ?
O7 As1 O13 Mo4 -56.2(4) . . . . ?
O13 As1 O13 Mo5 -179.7(4) 2_655 . . . ?
O7 As1 O13 Mo5 -60.0(4) 2_655 . . . ?
O7 As1 O13 Mo5 60.7(4) . . . . ?
O13 As1 O13 Mo6 -63.2(3) 2_655 . . . ?
O7 As1 O13 Mo6 56.4(4) 2_655 . . . ?
O7 As1 O13 Mo6 177.1(3) . . . . ?
O21 Mo4 O13 As1 -152.4(11) . . . . ?
O14 Mo4 O13 As1 38.1(4) . . . . ?
O15 Mo4 O13 As1 136.0(4) . . . . ?
O19 Mo4 O13 As1 -125.5(4) . . . . ?
O20 Mo4 O13 As1 -48.2(3) 2_655 . . . ?
V2 Mo4 O13 As1 -84.5(3) . . . . ?
O21 Mo4 O13 Mo5 74.6(13) . . . . ?
O14 Mo4 O13 Mo5 -94.9(2) . . . . ?
O15 Mo4 O13 Mo5 3.0(2) . . . . ?
O19 Mo4 O13 Mo5 101.5(2) . . . . ?
O20 Mo4 O13 Mo5 178.8(2) 2_655 . . . ?
V2 Mo4 O13 Mo5 142.49(16) . . . . ?
O21 Mo4 O13 Mo6 -14.6(13) . . . . ?
O14 Mo4 O13 Mo6 175.9(2) . . . . ?
O15 Mo4 O13 Mo6 -86.2(2) . . . . ?
O19 Mo4 O13 Mo6 12.35(19) . . . . ?
O20 Mo4 O13 Mo6 89.6(2) 2_655 . . . ?
V2 Mo4 O13 Mo6 53.34(13) . . . . ?
O17 Mo5 O13 As1 -178.0(17) . . . . ?
O5 Mo5 O13 As1 42.4(3) 2_655 . . . ?
O12 Mo5 O13 As1 -43.3(3) . . . . ?
O16 Mo5 O13 As1 134.8(4) . . . . ?
O15 Mo5 O13 As1 -134.8(4) . . . . ?
O17 Mo5 O13 Mo4 -46.1(18) . . . . ?
O5 Mo5 O13 Mo4 174.3(2) 2_655 . . . ?
O12 Mo5 O13 Mo4 88.7(2) . . . . ?
O16 Mo5 O13 Mo4 -93.2(2) . . . . ?
O15 Mo5 O13 Mo4 -2.8(2) . . . . ?
O17 Mo5 O13 Mo6 50.2(18) . . . . ?
O5 Mo5 O13 Mo6 -89.5(2) 2_655 . . . ?
O12 Mo5 O13 Mo6 -175.1(2) . . . . ?
O16 Mo5 O13 Mo6 3.0(2) . . . . ?
O15 Mo5 O13 Mo6 93.4(2) . . . . ?
O18 Mo6 O13 As1 150.1(11) . . . . ?
O11 Mo6 O13 As1 -38.4(4) 2_655 . . . ?
O16 Mo6 O13 As1 -135.9(4) . . . . ?
O20 Mo6 O13 As1 48.0(3) . . . . ?
O19 Mo6 O13 As1 125.3(4) . . . . ?
O18 Mo6 O13 Mo4 12.4(13) . . . . ?
O11 Mo6 O13 Mo4 -176.1(2) 2_655 . . . ?
O16 Mo6 O13 Mo4 86.4(2) . . . . ?
O20 Mo6 O13 Mo4 -89.7(2) . . . . ?
O19 Mo6 O13 Mo4 -12.4(2) . . . . ?
O18 Mo6 O13 Mo5 -77.2(12) . . . . ?
O11 Mo6 O13 Mo5 94.4(2) 2_655 . . . ?
O16 Mo6 O13 Mo5 -3.1(2) . . . . ?
O20 Mo6 O13 Mo5 -179.2(2) . . . . ?
O19 Mo6 O13 Mo5 -101.9(2) . . . . ?
O21 Mo4 O14 Mo3 130.5(8) . . . . ?
O15 Mo4 O14 Mo3 -125.2(8) . . . . ?
O19 Mo4 O14 Mo3 -17.3(12) . . . . ?
O20 Mo4 O14 Mo3 31.7(8) 2_655 . . . ?
O13 Mo4 O14 Mo3 -51.7(8) . . . . ?
V2 Mo4 O14 Mo3 19.6(9) . . . . ?
O10 Mo3 O14 Mo4 -134.6(8) . . . . ?
O11 Mo3 O14 Mo4 -31.2(8) . . . . ?
O9 Mo3 O14 Mo4 124.1(8) . . . . ?
O6 Mo3 O14 Mo4 47.8(12) . . . . ?
O7 Mo3 O14 Mo4 53.0(8) . . . . ?
O21 Mo4 O15 Mo5 -172.9(4) . . . . ?
O14 Mo4 O15 Mo5 81.1(4) . . . . ?
O19 Mo4 O15 Mo5 -72.4(4) . . . . ?
O20 Mo4 O15 Mo5 -15.1(9) 2_655 . . . ?
O13 Mo4 O15 Mo5 -4.4(3) . . . . ?
V2 Mo4 O15 Mo5 -58.9(4) . . . . ?
O17 Mo5 O15 Mo4 177.9(4) . . . . ?
O5 Mo5 O15 Mo4 -2.4(9) 2_655 . . . ?
O12 Mo5 O15 Mo4 -79.6(4) . . . . ?
O16 Mo5 O15 Mo4 77.3(4) . . . . ?
O13 Mo5 O15 Mo4 4.5(3) . . . . ?
O18 Mo6 O16 Mo5 172.7(4) . . . . ?
O11 Mo6 O16 Mo5 -80.5(4) 2_655 . . . ?
O20 Mo6 O16 Mo5 14.7(9) . . . . ?
O19 Mo6 O16 Mo5 72.6(4) . . . . ?
O13 Mo6 O16 Mo5 4.6(3) . . . . ?
O17 Mo5 O16 Mo6 -177.6(4) . . . . ?
O5 Mo5 O16 Mo6 78.8(4) 2_655 . . . ?
O12 Mo5 O16 Mo6 0.1(9) . . . . ?
O15 Mo5 O16 Mo6 -77.1(4) . . . . ?
O13 Mo5 O16 Mo6 -4.7(3) . . . . ?
O22 V2 O19 Mo6 -117.60(18) . . . . ?
O20 V2 O19 Mo6 120.8(3) 2_655 . . . ?
O20 V2 O19 Mo6 3.7(2) . . . . ?
O19 V2 O19 Mo6 62.40(18) 2_655 . . . ?
Mo6 V2 O19 Mo6 101.97(19) 2_655 . . . ?
Mo4 V2 O19 Mo6 124.6(3) . . . . ?
Mo4 V2 O19 Mo6 22.8(3) 2_655 . . . ?
O22 V2 O19 Mo4 117.81(17) . . . . ?
O20 V2 O19 Mo4 -3.8(2) 2_655 . . . ?
O20 V2 O19 Mo4 -120.8(3) . . . . ?
O19 V2 O19 Mo4 -62.18(18) 2_655 . . . ?
Mo6 V2 O19 Mo4 -22.6(3) 2_655 . . . ?
Mo4 V2 O19 Mo4 -101.8(2) 2_655 . . . ?
O18 Mo6 O19 V2 93.7(3) . . . . ?
O11 Mo6 O19 V2 -55.2(6) 2_655 . . . ?
O16 Mo6 O19 V2 -163.5(3) . . . . ?
O20 Mo6 O19 V2 -3.5(2) . . . . ?
O13 Mo6 O19 V2 -91.5(2) . . . . ?
O18 Mo6 O19 Mo4 -157.9(3) . . . . ?
O11 Mo6 O19 Mo4 53.3(7) 2_655 . . . ?
O16 Mo6 O19 Mo4 -55.0(3) . . . . ?
O20 Mo6 O19 Mo4 104.9(3) . . . . ?
O13 Mo6 O19 Mo4 17.0(3) . . . . ?
O21 Mo4 O19 V2 -93.8(3) . . . . ?
O14 Mo4 O19 V2 54.5(6) . . . . ?
O15 Mo4 O19 V2 163.5(3) . . . . ?
O20 Mo4 O19 V2 3.5(2) 2_655 . . . ?
O13 Mo4 O19 V2 91.6(2) . . . . ?
O21 Mo4 O19 Mo6 157.6(3) . . . . ?
O14 Mo4 O19 Mo6 -54.1(7) . . . . ?
O15 Mo4 O19 Mo6 54.9(3) . . . . ?
O20 Mo4 O19 Mo6 -105.1(3) 2_655 . . . ?
O13 Mo4 O19 Mo6 -17.0(3) . . . . ?
V2 Mo4 O19 Mo6 -108.6(4) . . . . ?
O22 V2 O20 Mo6 101.4(2) . . . . ?
O20 V2 O20 Mo6 -78.6(2) 2_655 . . . ?
O19 V2 O20 Mo6 -152.9(3) 2_655 . . . ?
O19 V2 O20 Mo6 -3.8(2) . . . . ?
Mo6 V2 O20 Mo6 -118.3(2) 2_655 . . . ?
Mo4 V2 O20 Mo6 -38.5(2) . . . . ?
Mo4 V2 O20 Mo6 -156.7(4) 2_655 . . . ?
O22 V2 O20 Mo4 -101.9(2) . . . 2_655 ?
O20 V2 O20 Mo4 78.1(2) 2_655 . . 2_655 ?
O19 V2 O20 Mo4 3.8(2) 2_655 . . 2_655 ?
O19 V2 O20 Mo4 152.9(3) . . . 2_655 ?
Mo6 V2 O20 Mo4 38.4(2) 2_655 . . 2_655 ?
Mo4 V2 O20 Mo4 118.1(2) . . . 2_655 ?
O18 Mo6 O20 V2 -93.6(3) . . . . ?
O11 Mo6 O20 V2 161.9(3) 2_655 . . . ?
O16 Mo6 O20 V2 64.6(7) . . . . ?
O19 Mo6 O20 V2 3.8(2) . . . . ?
O13 Mo6 O20 V2 74.3(3) . . . . ?
O18 Mo6 O20 Mo4 127.7(5) . . . 2_655 ?
O11 Mo6 O20 Mo4 23.2(5) 2_655 . . 2_655 ?
O16 Mo6 O20 Mo4 -74.1(8) . . . 2_655 ?
O19 Mo6 O20 Mo4 -135.0(6) . . . 2_655 ?
O13 Mo6 O20 Mo4 -64.4(5) . . . 2_655 ?

_diffrn_measured_fraction_theta_max 0.998
_diffrn_reflns_theta_full        25.08
_diffrn_measured_fraction_theta_full 0.998
_refine_diff_density_max         1.729
_refine_diff_density_min         -1.853
_refine_diff_density_rms         0.201


